FACULTE DES SCIENCES

J¨ulich Centre for Neutron Science JCNS und Peter Gr¨unberg Institut PGI JCNS-2, PGI-4: Scattering Methods ”Lattice Dynamics in Emerging Functional Materials” group Forschungszentrum J¨ulich

Lattice dynamics in thermoelectric Zintl phases

Ann´eeacad´emique2010–2011 Dissertation pr´esent´eepar Anne M¨ochel en vue de l’obtention du grade de Docteur en Sciences

Acknowledgements

My very ﬁrst gratitude goes to Dr. Rapha¨elP. Hermann for advising and supporting me during my doctoral thesis and for the fruitful discussions.

My special thanks go to my co-supervisor Dr. Werner Schweika, for his suggestions and especially for his comments on and the correction of this dissertation.

I would also like to thank my co-advisor at the University Li`egeProf. R. Cloots. I thank Prof. J.-P. Gaspard and Dr. W. Schweika for accepting to be in my thesis advisory comit- tee and Prof. B. Vertruyen, Prof. M. Verstraete and Dr. Ilya Sergueev for accepting to be members of the examination jury.

Many people collaborated to this work and I would like to specially thank Mr. D. Bessas, Dr. S. Disch, Dr. A. Houben, Dr. F. Juranyi, Dr. D. Robinson, Dr. K. Schmalzl, Dr. W. Schmidt, Dr. I. Sergueev, Dr. M. B. Stone, Dr. J. Voigt, Dr. H.-C. Wille, Prof. Th. Br¨uckel, Prof. F. Grandjean, Prof. D. C. Johnson, Prof. S. M. Kauzlarich, Prof. V. Keppens, Prof. Gary J. Long, Prof. A. Schengelaya and Prof. H. Schober for their help during experiments, for corrections and advises as well as for helpful discussions.

I would like to thank all my colleagues from the Institute of Scattering Methods and particularly Mr. B. Schmitz for his technical assistance.

For the funding of my PhD thesis I would like to acknowledge the Forschungszen- trum J¨ulich GmbH and the Helmholtz Association of German Research Centres, through to funding of the “Lattice Dynamics in Emerging Functional Materials” Investigator Group. I thank Prof. Th. Br¨uckel for ﬁnancial support at the beginning of my thesis.

The European Synchrotron Radiation Facility, the Advanced Photon Source, the Spalla- tion Neutron Source, the Paul Scherrer Institut, the Institut Laue-Langevin, the Forschungs- Neutronenquelle Heinz Maier-Leibnitz (FRM II) and the J¨ulich Centre for Neutron Science are acknowledged for provision of synchrotron and neutron beam time.

I want to particularly thank my parents for their support and conﬁdence.

Finally, I want to thank my boyfriend Andreas for his support, his technical assistance, his patience and his love.

I Publication Dissertation

Chapter 2−5 of this dissertation are manuscripts that are submitted or will be submitted shortly and formatted in RevTex4.

Chapter 2: A. M¨ochel, I. Sergueev, N. Nguyen, Gary J. Long, F. Grandjean, D. C. Johnson, and

R. P. Hermann, Lattice Dynamics in the FeSb3 Skutterudite, submitted to Phys. Rev. B, March 2011.

Chapter 3: A. M¨ochel, I. Sergueev, H.-C. Wille, J. Voigt, M. Prager, M. B. Stone, B. C. Sales, Z. Guguchia, A. Shengelaya, V. Keppens, and R. P. Hermann, Lattice dynamics and anomalous softening in the YbFe4Sb12 skutterudite, to be submitted to Phys. Rev. B, May 2011.

Chapter 4: A. M¨ochel, W. Schweika, K. Schmalzl, B. C. Sales, and R. P. Hermann, Experimental study of the phonon dispersion in the Sr8Ga16Ge30 clathrate, to be submitted to New Journ. Phys., June 2011.

Chapter 5: A. M¨ochel, I. Sergueev, H.-C. Wille, F. Juranyi, H. Schober, W. Schweika, S. R. Brown, S. M. Kauzlarich, and R. P. Hermann, Lattice dynamics in the thermoelectric Zintl compound Yb14MnSb11, to be submitted to Phys. Rev. B, May 2011.

II Abstract

A brief introduction to the thermoelectric eﬀects, the studied materials, and the experimen- tal methods is given in the ﬁrst chapter. The introduction is not intended to be exhaustive, but only to summarize important basic information for the reader. The introduction is followed by four chapters dedicated to detailed experimental studies of the lattice dynamics in selected thermoelectric Zintl phases.

First, the lattice dynamics in the unﬁlled and ﬁlled skutterudites FeSb3, CoSb3, and

YbFe4Sb12 were studied by nuclear inelastic scattering, inelastic neutron scattering, and several macroscopic methods. These studies reveal that FeSb3 exhibits softer Sb bonds than

CoSb3, that the density of phonon states is shifted towards lower energies and the velocity of sound is lower in FeSb3 as compared to CoSb3. It appears thus that the soft [Fe4Sb12] framework dynamics might play an important role in the thermoelectric properties of ﬁlled skutterudites. The observed anomalous temperature dependence of the elastic constants and the rearrangement of the spectral weight of the Yb phonon states in YbFe4Sb12 can be explained by a change of the Yb valence state with the temperature.

Second, the lattice dynamics in the Sr8Ga16Ge30 clathrate was investigated by inelastic neutron scattering measurements on a single crystal. We found that several mechanisms contribute to the low thermal conductivity in this system and that the reduction of the heat capacity contribution to the thermal conductivity plays a signiﬁcant role to the low thermal conductivity, besides the reduction in the phonon lifetime and the phonon group velocity that is related to the guest atom.

Third, the lattice dynamics of the Zintl phase Yb14MnSb11 was studied by inelastic neu- tron scattering and nuclear inelastic scattering measurements. All phonon modes of these complex crystal systems are in a narrow energy range below ∼25 meV and the Debye tem- perature, the velocity of sound and the mean force constants are small compared to those of other thermoelectric materials such as Zn4Sb3. By comparing the lattice dynamics in

Yb14MnSb11 and Zn4Sb3 diﬀerent mechanisms which lead to the low thermal conductivity in Zintl phases have been identiﬁed. Between 300 and 1200 K no softening of the velocity of sound in Yb14MnSb11 was observed by temperature dependent inelastic neutron scattering measurements, which is in line with its large melting temperature.

III R´esum´e

Le premier chapitre introduit bri`evement les eﬀets thermo´electriques,les mat´eriaux´etudi´es et les techniques exp´erimentales utilis´ees.Cette introduction ne se veut pas exhaustive, mais r´esumeseulement les informations essentielles pour le lecteur. Cette introduction est suivie de quatre chapitres d´edi´esaux ´etudesexp´erimentales d´etaill´eesdes la dynamique de r´eseau dans une s´electionde phases de Zintl thermo´electriques.

Premi`erement, la dynamique de r´eseaudans les skutt´eruditesvides et remplies FeSb3,

CoSb3, et YbFe4Sb12 ont ´et´e´etudi´eespar diﬀusion nucl´eairer´esonante in´elastique, diﬀusion in´elastiquede neutrons ainsi que diverses techniques macroscopiques. Ces ´etudesr´ev`elent que FeSb3 poss`edent des liaisons de Sb plus faibles que dans CoSb3 et que par ce fait, la densit´ed’´etats de phonons est d´eplac´eesvers des ´energiesplus faibles et que la vitesse du son dans FeSb3 est r´eduitepar rapport `aCoSb3. Il apparaˆıtdonc que la dynamique de l’ossature structurelle [Fe4Sb12] puisse jouer un rˆoleimportant dans les skutt´erudites remplies. La d´ependance en temp´eratureanomale des constantes ´elastiqueset le r´earrangement du poids spectral des ´etatsde phonons de Yb dans YbFe4Sb12 a ´et´e´etudi´eet peut s’expliquer par une modiﬁcation de l’´etatde valence de Yb en fonction de la temp´erature.

Deuxi`emement, la dynamique de r´eseaudans la clathrate Sr8Ga16Ge30 a ´et´e´etudi´ee par diﬀusion in´elastiquede neutrons sur un monocristal. Nous avons mis en ´evidenceque plusieurs m´ecanismes contribuent `ala faible conductivit´etechnique dans ce syst`emeet que la r´eductionde la chaleur sp´eciﬁquepartielle contribuant `ala conductivit´ethermique joue un rˆolesigniﬁcatif pour la faible conductivit´ethermique, `acˆot´ede la r´eductiontant du temps de vie des phonons que de leur vitesse de groupe, une r´eduction li´eeaux atomes hˆotes.

Troisi`emement, la dynamique de r´eseaude la phase de Zintl Yb14MnSb11 a ´et´e´etudi´eepar diﬀusion in´elastiquede neutrons et diﬀusion nucl´eairein´elastique. Tous les modes de phonons de cette structure cristalline complexe se trouvent dans un bande d’´energie´etroite en de¸c`a de ∼25 meV et que la temp´eraturede Debye, la vitesse du son et les constantes de forces moyennes sont faibles par rapport `ad’autres mat´eriaux thermo´electriques, tels que Zn4Sb3. Par comparaison, les m´ecanismesdiﬀ´erents qui contribuent `ala faible conductivit´edans les phases de Zintl Yb14MnSb11 et Zn4Sb3 ont ´et´e´etudi´es.Aucune r´eductionsigniﬁcative de la vitesse du son dans Yb14MnSb11 entre 300 et 1200 K n’a ´et´eobserv´eepar diﬀusion in´elastique de neutrons, ce qui est en accord avec la temp´eraturede fusion ´elev´ede ce mat´eriau.

IV Kurzbeschreibung

Im ersten Kapitel ist eine kurze Einleitung zu den thermoelektrischen Eﬀekten, den unter- suchten Materialien und den experimentellen Methoden gegeben. Diese Einleitung erhebt keinen Anspruch auf Vollst¨andigkeit und sie ist als eine kurze Einf¨uhrungin die Grundlagen f¨urden Leser gedacht. Der Einleitung folgen vier Kapitel welche den detailierten experi- mentellen Studien zu der Gitterdynamik in thermoelektrischen Zintl Phasen gewidmet sind.

Erstens: Die Gitterdynamik wurde in den ungef¨ulltenund gef¨ulltenSkutteruditen FeSb3,

CoSb3 und YbFe4Sb12 mit Hilfe der inelastischen Kernresonanz, der inelastischen Neutro- nenstreuung und unterschiedlichen makroskopischen Messmethoden untersucht. Diese Un- tersuchungen zeigen, dass FeSb3 weichere Sb Bindungen aufweist als CoSb3, die Phononen- zustandsdichte zu tieferen Energien hin verschoben ist und die Schallgeschwindigkeit in

FeSb3 niedriger als in CoSb3 ist. Daher scheint die Dynamik der [Fe4Sb12] Grundstruktur eine wichtige Rolle f¨urdie thermoelektrischen Eigenschaften in gef¨ulltenSkutteruditen zu spielen. Der anomale Temperaturverlauf der elastischen Konstanten und die Umordnung der

Yb Phononenzust¨andein der Phononenzustandsdichte von YbFe4Sb12 wurden untersucht und k¨onnendurch die temperaturabh¨angige Anderung¨ des Yb Valenzzustandes erkl¨artwer- den.

Zweitens: Die Gitterdynamik des Sr8Ga16Ge30 Clathrates wurde durch inelastische Neu- tronenstreumessungen an einem Einkristall untersucht. Es wurde herausgefunden, dass verschiedene Mechanismen f¨urdie niedrige thermische Leitf¨ahigkeit dieses Systemes ver- antwortlich sind und dass die Reduzierung des W¨armekapazit¨atsbeitrages zu der thermisch- en Leitf¨ahigkeit, neben der Reduzierung der Phononenlebenszeit und der Phononengrup- pengeschwindigkeit durch das Gastatom, ein weiterer wichtiger Faktor f¨urdie niedrige thermische Leitf¨ahigkeit ist.

Drittens: Die Gitterdynamik der Zintl Phase Yb14MnSb11 wurde durch inelastische Neu- tronenstreuung und inelastische Kernresonanzmessungen untersucht. Alle Phononenmoden dieses komplexen Kristallsystems liegen in einem Energiebereich unterhalb von ∼25 meV und die Debyetemperatur, die Schallgeschwindigkeit und die mittleren Kraftkonstanten sind

niedrig im Vergleich zu anderen thermoelektrischen Materialien wie Zn4Sb3. Durch den Ver-

gleich der Gitterdynamik in Yb14MnSb11 zu der in Zn4Sb3 wurden die unterschiedlichen Mechanismen, welche zu den niedrigen thermischen Leitf¨ahigkeiten in Zintl Phasen f¨uhren, bestimmt. In den temperaturabh¨angigen inelastischen Neutronenstreumessungen wurde f¨ur

Yb14MnSb11 keine Erniedrigung der Schallgeschwindigkeit zwischen 300 und 1200 K fest- gestellt, was in guter Ubereinstimmung¨ mit der hohen Schmelztemperatur ist.

V Contents i Contents

AcknowledgementsI

Publication DissertationII

AbstractIII

R´esum´eIV

KurzbeschreibungV

General Introduction2

I. Thermoelectricity2

II. Zintl Formalism3

III. Studied Materials4 A. Skutterudites4 B. Clathrates6

C. Yb14MnSb11 7

IV. Macroscopic Measurements8 A. Heat Capacity Measurements8 B. Magnetization and Resistivity Measurements 10 C. Resonant Ultrasound Spectroscopy 11

V. Elastic Scattering and Diﬀraction 12

VI. Inelastic Scattering 14 A. Inelastic Neutron Scattering 16 B. Nuclear Inelastic Scattering 19

References 23 Contents ii

Lattice Dynamics in the FeSb3 Skutterudite 26

Abstract 26

I. Introduction 27

II. Experimental 28

III. Results and discussion 30 A. Electric transport and magnetism 30 B. X-ray diﬀraction 33 C. M¨ossbauerspectroscopy 36 D. Nuclear resonance scattering 39

IV. Conclusion 46

Acknowledgments 47

References 47

Lattice dynamics and anomalous softening in the YbFe4Sb12 skutterudite 51

Abstract 51

I. Introduction 52

II. Experimental 54

III. Results and discussion 55 A. Resonant ultrasound spectroscopy 55 B. Structure and magnetism 57 C. M¨ossbauerspectroscopy 61 D. Inelastic neutron scattering 62 E. Nuclear inelastic scattering 63 F. Valence state 70

IV. Conclusion 71

Acknowledgments 72

References 72 Contents iii

Experimental study of the phonon dispersion in the

Sr8Ga16Ge30 clathrate 76

Abstract 76

I. Introduction 77

II. Experimental 79

III. Results and discussion 79 A. Phonon lifetime 82 B. Phonon velocity 84 C. Model 85 D. Anharmonicity 87

IV. Conclusion 90

Acknowledgments 91

References 92

Lattice dynamics in the thermoelectric Zintl compound

Yb14MnSb11 95

Abstract 95

I. Introduction 96

II. Experimental 99

III. Results and discussion 99 A. Structure 99 B. Density of phonon states 103

IV. Conclusion 115

Acknowledgments 115

References 116

Conclusions and Outlook 119

Vita 122 Chapter 1

General Introduction

1 Chapter 1: General Introduction – Thermoelectricity 2

This introduction is not intended to be exhaustive, but only to summarize important basic information for the reader. General references for the sections are indicated next to the section title.

I. THERMOELECTRICITY1–4

The environmentally friendly generation and conversion of energy is an important task due to our increasing power consumption and its large inﬂuence on the climate related to conventional methods of fossil energy conversion. Thermoelectric materials can be used to convert heat into electricity by harnessing the Seebeck eﬀect. Conversely, cooling can be achieved via the Peltier eﬀect. The functionality of a thermoelectric couple, which is used in thermoelectric devices, is illustrated in Fig.1: Thermoelectric couples consist of two semi- conducting legs, namely one that transports negative charges (n-type) and the other one that transports positive charges (p-type). The semiconducting legs possess a diﬀerence in the Fermi energy. Thus, the charge carriers have diﬀerent transport energies in the diﬀerent legs. If a current passes from one leg to the other, the transported energy of the carriers is modiﬁed and the diﬀerence appears as heating or cooling in the junction. Conversely, if the junction is heated, the carriers can pass from one material with lower carrier energy to the other material with higher carrier energy. This yields an electromotive force and in a closed circuit a current ﬂows. A good thermoelectric material has to possess a good electrical con- ductivity and a small thermal conductivity, because its eﬃciency is proportional to the ﬁgure of merit, ZT = σα2T/κ, with the electrical conductivity, σ, the material dependent Seebeck coeﬃcient, α, and the thermal conductivity κ. Thus, a good thermoelectric material should both behave as an electron crystal and a phonon glass5. Nowadays, Peltier elements are mainly used in applications, where noiseless, cryogen gas free or space saving cooling devices or bipolar cooling are requested, e.g. in minibar fridges or sample array coolers in biology. For energy conversion, thermoelectric devices are used, if a compact and maintenance free device is needed, e.g. in spacecrafts. The potential use as converter of waste heat, e.g. for recovering energy from the exhaust gas of an automobile, into electricity has only prototype value today, due to the low eﬃciency of the state of the art thermoelectric devices. One way to increase the ZT and therefore the eﬃciency, is to reduce the thermal conductivity without changing the electrical properties. In a semiconductor, heat is transported by electrical car- Chapter 1: General Introduction – Zintl Formalism 3 riers and phonons, i.e. the thermal conductivity has an electrical and a lattice contribution. PbTe and SiGe, which are common thermoelectric materials used today, exhibit thermal conductivities of ∼2.2 W/(m K) at 300 K and ∼3.5 W/(m K) at 900 K, respectively6,7 and possess a ZT value of ∼0.8 and ∼0.4, respectively, at the indicated temperatures7. In order to achieve a high ZT value, the lattice part of the thermal conductivity has to be reduced. Because the electrical part is strongly dependent on the electrical resistivity, a lowering of the electrical thermal conductivity would also lead to a lowering of the electrical resistiv- ity and the ZT value would not be enhanced. In the simple kinetic gas theory, the lattice thermal conductivity is dependent on the speciﬁc heat capacity, CV , the mean velocity of sound, vs, and the mean free path of the phonons, λ: κL = CV vsλ/3. One approach of low- ering the lattice thermal conductivity in bulk materials is the ﬁlling of cage structures, e.g. skutterudites or clathrates, with heavy atoms, such as Yb, Sb or Eu. The dynamics of the ﬁller impedes the thermal transport by reducing the mean free path of the phonons as well as the mean phonon velocity, and both eﬀects contribute to a lower thermal conductivity. Another approach is the use of complex crystal systems with a large number of atoms in the unit cell, e.g. Yb14MnSb11, where the contribution of the heat capacity to the thermal conductivity is reduced. Nanostructuring, nanoinclusions and lowering the dimensionality are other approaches to reduce the thermal conductivity by phonon conﬁnement. This work is focused on a detailed experimental study of the lattice dynamics in thermoelec- tric bulk Zintl phases, in order to investigate the mechanisms that lead to the low thermal conductivity as observed in these systems.

II. ZINTL FORMALISM8

Zintl phases are intermetallic compounds of electropositive metals, such as alkaline, al- kaline earth and lanthanides, and metals with a medium electronegativity. The cations are electron donors to the anionic sublattice. The typically larger anions form the structure and generates subunits, i.e. polyanions, similar to the isoelectronical pure elements, e.g. in the compound NaTl the [Tl−] anions are forming a diamond structure in which the Na+ ions are located. Zintl phases most often obey the general valence rule. The rich chemistry of Zintl phases oﬀers numerous possibilities for chemical substitutions and structural modiﬁ- cations that allows the tuning of the fundamental transport parameters in order to improve Chapter 1: General Introduction – Studied Materials 4

Heat source

Refrigeration Active cooling

p n p n Current

Heat sink Heat sink

– +

External power input Power conversion

FIG. 1. Illustration of the Peltier, left, and Seebeck eﬀect, right, in a thermoelectric couple [2]. the thermoelectric performance9. Herein, the following compounds, which obey the Zintl formalism, are studied: a) Skutterudites: In the unﬁlled skutterudite FeSb3 the unit cell contains 8 formula units and consist of a network of corner sharing [FeSb6] octahedrals. Fe has a formal valence state of 3+ whereas Sb has a formal valence state10 of 1−. By ﬁlling the structure with Yb, which has a valence state of 2+ at 300 K, the average Fe valence state is lowered to 2.5+ in the

YbFe4Sb12 compound. The valence state of the Sb anionic sublattice does not change. b) 1− 0 Clathrates: In Sr8Ga16Ge30 the unordered polyanions consisting of Ga and Ge form two types of cages1, namely a dodecahedron of 20 Ga and Ge atoms and a tetrakaidecahedron 2+ of 24 Ga and Ge atoms. The Sr is located in both cage types. c) Yb14MnSb11: The struc- 9− 7− 3− ture is generated by 8 units of a MnSb4 tetrahedron, a Sb3 polyanion and 4 Sb anions, whereas the Yb2+ are donating 28 electrons11.

III. STUDIED MATERIALS

A. Skutterudites

Skutterudites, see Fig.2, have 1 cubic crystal structure with the space group Im3. The archetype material is the mineral (Co,Ni)As3. Skutterudites are promising thermoelectric materials due to the possibility of tuning the thermal properties by ﬁlling the cage structure Chapter 1: General Introduction – Studied Materials 5

with only slight changes of the electronic properties12 and the typical thermal stability up 13,14 to ∼800 K. It was suggested that by ﬁlling the skutterudite framework, [Co4Sb12] or

[Fe4Sb12], with lanthanides, such as La, Eu of Yb, which have large masses in comparison to the host atoms, the thermal conductivity will be reduced. This reduction of the ther- mal conductivity, κ, by ﬁlling the structure with heavy elements was veriﬁed14,15 in several compounds, e.g. in La0.3Co4Sb12 and CeFe0.75Co3.25Sb12, which shows a reduction of the thermal conductivity by 78% and 85%, respectively, compared to the unﬁlled compound

CoSb3. The precise mechanism behind the reduction in κ caused by the ﬁller in skutteru- dites and clathrates, see below, is still an open question. One suggestion for the reduction mechanism of the thermal conductivity was that the ’rattling’ of the ﬁller compound has an inﬂuence on the lattice dynamics of the host structure16: The phonon mean free path is reduced by the movement of the ﬁller and therefore the thermal conductivity is reduced. Another suggestion for the reduction of the thermal conductivity is that through the inter- action of the guest and the host modes the acoustic phonon modes are ﬂattened and due to this avoided crossing the velocity of sound is reduced17. It was also suggested that the interaction of the low energy optical guest modes and the acoustic phonon modes lead to Umklapp scattering, which hinders the heat transport18, but that otherwise skutterudites behave as a conventional phonon crystal and not as a phonon glass. Another approach to increase the ZT value is the enhancement of the electrical properties by doping12. This will not be regarded in this work.

FIG. 2. The unﬁlled (left) and ﬁlled (right) skutterudite structure. Blue, red and yellow indicates Sb, Fe or Co and the ﬁller R, respectively. Chapter 1: General Introduction – Studied Materials 6

In this work the lattice dynamics in the ﬁlled and unﬁlled skutterudites, YbFe4Sb12 and 19 FeSb3, respectively, were studied. Due to the poor electrical properties, YbFe4Sb12 exhibits a low ZT value of ∼0.02 at 300 K. Nevertheless, because of the low thermal conductivity of 2 W/(m K) at 300 K19 it is a useful model system for investigating the inﬂuence of the ﬁller on the thermal conductivity. In the temperature dependence of the elastic constants of

YbFe4Sb12, an anomaly was found at ∼50 K and the reason of this anomaly is likely a change of the Yb valence state with temperature, see Chapter 3. The unﬁlled parent compound 20 FeSb3 is metastable and can be prepared only as ﬁlms, see Chapter 2. The synthesis of a pure phase ﬁlm was recently successful and the structure, the electrical conductivity,

the magnetism and the lattice dynamics were studied. This study reveals that FeSb3 is softer in the lattice dynamics than the isostructural compound CoSb3, see Chapter 2. The characterization of the Seebeck coeﬃcient and the thermal conductivity could not carried out so far, therefore a ZT value is not available.

B. Clathrates

Clathrates are host-guest complexes1,8 and the two archetypes have the general formula

X2Y6E46 (type I), e.g. Sr8Ga16Ge30, and X8Y16E136 (type II), e.g. Na3Si136 [21], where X and Y are the guest atoms, while the E atoms are forming the host structure. In this work, the lattice dynamics in the type I clathrate Sr8Ga16Ge30 were studied. The same mechanisms behind the low thermal conductivity in clathrates were suggested as for skutterudites, see above. The comparison with an unﬁlled system is not possible in this case, because the unﬁlled Ga-Ge clathrate is structurally unstable without the ﬁller atom22, however recently empty Si and Ge chlatrates have been synthesized23 and further studies on their lattice dy-

namics will certainly be of high interest. Sr8Ga16Ge30 crystallizes in the cubic space group

P m3n, see Fig.3. Other isostructural systems exist such as Ba 8Ga16Ge30 and Na8Si46, which are also candidates for thermoelectric applications. Sr can occupy the center of two diﬀerent cages, the smaller dodecahedron of 20 Ga and Ge atoms and the larger tetrakaidecahedron of 24 Ga and Ge atoms. It was found24 that the Sr atoms sitting in the larger cage play 25 the predominant role in the reduction of the thermal conductivity. Sr8Ga16Ge30 exhibits a thermal conductivity of 1 W/(m K) at 300 K. With the electrical resistivity and the Seebeck coeﬃcient26 of ρ = 2 mΩ cm and S = −115 µV/K, respectively, at room temperature, a Chapter 1: General Introduction – Studied Materials 7

FIG. 3. The crystal structure of the Sr8Ga16Ge30 clathrate. Yellow indicates Ga and Ge and blue and red the Sr atom sitting in the smaller and larger cage, respectively.

modest ZT of 0.02 was obtained for Sr8Ga16Ge30. In order to investigate the lattice dy- namics in Sr8Ga16Ge30, the phonon dispersion was studied by inelastic neutron scattering measurements on a single crystal and the ﬁndings are summarized in Chapter 4. It was found that beside the reduction of the phonon lifetime and the phonon velocity by the inﬂuence of the guest atom the lowering of the heat capacity of the acoustic phonons and thus the heat capacity contribution to the thermal conductivity is also an important mechanism, which yields to the low thermal conductivity in Sr8Ga16Ge30.

C. Yb14MnSb11

11 The Zintl phase Yb14MnSb11 crystallizes in the tetragonal space group I41/ a c d. The large unit cell of ∼6060 A˚ consists of 208 atoms, see Fig.4. This material exhibits 27 a nearly temperature independent low thermal conductivity of 0.8 W/(m K) between 300 and 1200 K, which is in the range of the thermal transport coeﬃcient of glasses. Combined with the good electrical properties above 900 K a ZT value of 0.8 at 1000 K is observed. Furthermore, the material stays solid up to ∼1300 K, which makes this system a promising candidate for ther- moelectric applications in the high temperature range, e.g. for radioisotope thermoelectric generators as used in spacecrafts. It was suggested9 that one reasons for the low thermal conductivity is the small contribution of the heat capacity to the thermal conductivity, due Chapter 1: General Introduction – Macroscopic Measurements 8

FIG. 4. Crystal structure of Yb14MnSb11. The red, blue and green spheres represent the Yb, Sb and Mn atoms, respectively. to the large unit cell volume. The heat capacity is equally divided to all phonon modes and because of the small optical phonon velocity, the heat transport is mainly through the acoustic phonons. Due to the small ratio of acoustic to optical modes in Yb14MnSb11 com- pared to systems with a smaller number of atoms in the unit cell, the contribution of the heat capacity to the thermal conductivity is low. Furthermore, it was empirical derived9,28

that in structures, which exhibit a large diﬀerence in the atom masses, such as Yb14MnSb11, the heat transport through the optical modes can be neglected. The lattice dynamics were studied in this system and the results are summarized in Chapter 5. It was found that an- other important mechanism which lead to the low thermal conductivity in this system, is the low velocity of sound, beside the reduction of the heat capacity contribution to the thermal conductivity.

IV. MACROSCOPIC MEASUREMENTS

A. Heat Capacity Measurements3

Speciﬁc heat capacity measurements at constant pressure, CP , were done using a physical properties measurement system from Quantum Design (QD-PPMS) with a commercially available setup29. The sample holding puck is shown in Fig.5. The platform is connected Chapter 1: General Introduction – Macroscopic Measurements 9

FIG. 5. The setup of the puck for measuring the heat capacity, from Ref. [29], and a photo of the puck.

to the frame of the puck by 8 wires. A small amount of grease between sample and the platform guarantees the thermal contact. During the measurements, the puck is in high- vacuum of ∼10−5 mbar. Therefore, the only thermal connection to the platform are the wires. To measure the heat capacity, a heat pulse is applied to the platform, (heater in Fig.5) and therefore to the sample and the heat relaxation time of the platform with the sample is measured (thermometer in Fig.5). From the relaxation time of the platform with the sample, the heat capacity CP can be calculated in ﬁrst approximation by τ = CP /KW ,

with the inverse relaxation time τ and the thermal conductivity of the wires KW . In a more complete model, the non ideal coupling of the sample to the platform is considered and the heat capacity was corrected for this. The dominant contributions to the heat capacity of non-magnetic materials is the elec- tronic and the lattice vibration contribution. At low temperatures, the electronic contri- bution shows a linear dependence with the temperature, whereas the lattice contribution has a cubic dependence with the temperature. At elevated temperatures, the lattice con- tribution is the dominant part in the heat capacity. Lattice dynamical properties can be obtained from the heat capacity. There are two models for the lattice vibrations: In the Debye model it is assumed that all atoms move collectively and that the dependence of the frequency to the wavevector, ~k, of the collective motion, i.e. the phonons, is linear up to the Debye frequency. This approximation describes more or less accurately the acoustic

phonons, see below. The Debye frequency, ωD, is proportional to the Debye temperature

θD = ~ωD/kB. The underlying assumption of the Einstein model is that all atoms vibrate independently from each other with the same frequency, the Einstein frequency. This model

is an idealization of optical phonons. The Einstein temperature θE is proportional to the

Einstein frequency, ωE. The lattice part of the heat capacity has contributions both from Chapter 1: General Introduction – Macroscopic Measurements 10

the optical and the acoustic phonons and a combination of the Debye and Einstein models can be used for the heat capacity. In the Debye model, the speciﬁc heat can be expressed 3 R θD/T 4 2 ~ by: CV = 9nkB(T/θD) 0 x exp(x)dx/(exp(x) − 1) , with x = (~ck)/(kBT ), the speed of light, c, and the wavevector ~k. In the Einstein model, the speciﬁc heat is expressed by: 2 2 CV = pnkB(θET ) exp(θET )/(exp(θET ) − 1) , with the number of primitive cells per unit volume n and the number of optical branches p. From the temperature dependence of the heat capacity, the Debye and Einstein temperatures can be obtained. These models are only approximations but nevertheless the models are useful in order to compare diﬀerent materials and these models give an insight into the lattice dynamics.

B. Magnetization and Resistivity Measurements29

In order to precharacterize the samples, magnetization and resistivity measurements are useful, because the magnetism and the resistivity of a sample is strongly dependent on the phase, the microstructure and on impurities in the sample. Magnetization measurements were carried out on a QD-PPMS using the vibrating sample magnetometer, VSM, option. The VSM is a DC magnetometer with a sensitivity of ∼10−5 emu and a magnetic ﬁeld up to 9 T can be applied to the sample. The setup is shown in Fig.6. The sample vibrates between the pickup coils with a frequency of 40 Hz, inducing a voltage in the coils. The induced voltage is proportional to the magnetic moment of the sample. By changing the temperature or the applied magnetic ﬁeld, the susceptibility or the hysteresis of the sample can be measured. The obtained results have to be corrected for the diamagnetic contribution of the sample holder, see also Chapter 2. The electrical resistivity was measured with a commercially available option for a QD- PPMS using the four point method. A sketch of the sample holder setup, with which 3 samples can be measured at the same time, is shown in Fig.6. The four wires are connected to each sample by silver paint and to the sample holder by soldering the wires to the voltage and current contacts. Thin silver wires were used for the measurements in this work. A DC current is applied to the sample (I+ and I−) and the resulting voltage is measured between the V+ and V− contacts. The distance between the voltage contacts on the sample, l, and the cross section of the sample, A, has to be known, in order to calculated the speciﬁc electrical resistivity by ρ = V A/(Il). Chapter 1: General Introduction – Macroscopic Measurements 11

FIG. 6. The VSM setup and a photo of the motor, the sample holder and the coil puck (left) and the setup for resistivity measurements (right), from Ref. [29].

C. Resonant Ultrasound Spectroscopy

With the resonant ultrasound spectroscopy the elastic constants and therefore the velocity of sound can be measured30. The sample is clamped between two piezoelectric transducers, such that it has no other contact apart from the transducers, see Fig.7. One transducer emits ultrasound waves with frequencies in the MHz range. The other transducer acts as a receiver. If the incoming wave has a frequency which is a full body resonance of the sample, a strong response signal is recorded. In the approximation of a homogeneous sample the resonant frequencies of the sample depend on the elastic constants, the density, and the geometry of the sample. By tuning the incoming frequency, various resonant frequencies can be determined and with the knowledge of the density and the geometry of the sample, the elastic constants can be obtained by a ﬁt of the frequency spectrum. Diﬀerent ﬁnite element models for diﬀerent sample geometries, e.g. for parallelepiped-shaped, spherical and cylindrical samples exist. In order to minimize the error bars of the obtained elastic constants, the shape of the sample has to be as close as possible to the sample geometry used for the model, with a typical tolerance of less than 2% in any linear dimension or angle. From a measurement of a polycrystalline sample two independent elastic constants can be obtained, c11 and c44. The shear modulus,c44, is typically denoted as G. From c11 and c44 the 2 Young modulus, E = (3c44c11 − 4c44)/(c11 − c44), the Poisson ratio, ν = (E/(2G)) − 1, and Chapter 1: General Introduction – Elastic Scattering and Diﬀraction 12

FIG. 7. The setup for the resonant ultrasound spectroscopy [34]. the bulk modulus, B = E/(3(1−2ν)), can be obtained31. Furthermore, the isotropic average 2 of the longitudinal and the transversal velocity of sound can be obtained by vL = c11/ρ and 2 vT = c44/ρ, respectively, with ρ as the density of the material. The mean velocity of sound can 2 2 −1/3 be calculated by vs = (1/3 ∗ (2/vT + 1/vL)) . The velocity of sound is proportional to the thermal conductivity and an important parameter for the lattice dynamics, see Chapter 4. From single crystal sample measurements, all independent elastic constants can be obtained. By the temperature dependence of the elastic constants, magnetic or structural phase transitions and anomalies can be studied. The typical temperature dependence of the elastic constants can be described by a phenomenological Varshni model32. If an anomaly or a phase transition occurs, a dip or a kink will be observed in the temperature dependence. The temperature dependence of the elastic constants was studied33 in ﬁlled skutterudites and a deviation from the Varshni function was seen as a dip at 50 K. The reason for this anomaly is the dynamics of the ﬁller atom, which can be described as an Einstein oscillator. By taking the response of such a Einstein oscillator into account, the anomalous temperature dependence can be modeled33. This localized phonon mode was also observed in the density of phonon states measured by inelastic neutron scattering. Herein, the study of the elastic

constants and the density of phonon states of YbFe4Sb12 will be reported in Chapter 3.

V. ELASTIC SCATTERING AND DIFFRACTION3,35

In a scattering process, the scattering particle, e.g. neutrons, electrons or photons, are described by waves with the wavevector ~k = 2π/λ. The wavelength, λ, is equivalent to Chapter 1: General Introduction – Elastic Scattering and Diﬀraction 13

the energy, E, and the mass, m, of the particle by the de Broglie relation λ = h/(mv) = √ h/( 2mE), with the velocity v. For photons, where v = c, λ = hc/E. The scattering vector, ~ ~ ~ Q, is deﬁned by the diﬀerence between the incident and the ﬁnal wavevector, ki and kf , ~ ~ ~ respectively, by Q = kf − ki. In an elastic process, the absolute value of the wavevector ~ ~ is not changed, |ki| = |kf |. Scattering takes place, if the scattering vector is equal to an ~ ~ ~ ~ reciprocal lattice vector G, |Q| = |G| = 2 sin θ|kf | = 4π sin θ/λ. θ is the angle between the incident beam and the scattering plane and in an elastic scattering process the angle between the scattered beam and the scattering plane is equal to θ. With the distance between the scattering planes, d, and |Q~ | = 2π/d, Bragg’s law is obtained: nλ = 2d sin θ. In other words, constructive interference takes place, if the angle θ is chosen, so that the path diﬀerence between neighboring waves, which is related to d, is an integer multiple n of the incident wavelength, which means that the scattered waves are in phase and a diﬀraction maximum can be detected. From several d values of diﬀerent directions as given by the Miller indices h, k and l, the lattice parameters can be determined. For rectangular lattice systems, i.e. cubic, orthorhombic and tetragonal crystal systems, the formula d = 1/(p(h2/a2 + k2/b2 + l2/c2)) yields the lattice parameter a, b and c.

In a diﬀraction measurement, a broad θ range will be studied without an energy resolution. Reﬂections, which obey Bragg’s law for several h, k and l combinations, deﬁned by the space group of the material, arises at deﬁned angles. From the positions of the reﬂections the lattice parameter can be obtained. The intensity, I, of the reﬂections are proportional to the diﬀerential cross section, I ∼ (dσ/dΩ), with the cross section σ and the distribution angle Ω. Since the scattering does not take place on a point, but on an object with ﬁnite dimension, ~ ~ 2 a form factor, f(Q), has to be implied: (dσ/dΩ)total = (dσ/dΩ)point · |f(Q)| . For x-ray’s, which are scattered by the electron cloud of the atoms, the atomic form factor is deﬁned as the Fourier transformation of the charge distribution f(Q~ ) = R ρ(~r) exp(iQ~r~ )d3r, with the electron density ρ and the equilibrium position of the atoms ~r. If there are diﬀerent atoms in the unit cell, the structure factor is obtained by summing over the form factors of each atom in the unit cell with appropriate phase shift. Due to thermal motions, the atoms are vibrating around their positions ~r. If an atom is not on the equilibrium position, the condition for constructive interference is not fulﬁlled. Therefore, the intensity of these reﬂections can be lowered depending on the size of the thermal excitation, which is temperature dependent. This is taken into account by the Debye-Waller factor f 0(Q~ ) = f(Q~ ) · exp(−2π2u2/d2), Chapter 1: General Introduction – Inelastic Scattering 14

with the mean-square displacement u2. Therefore, from the position and intensity of the reﬂections, the positions of the atoms in the unit cell, the occupation of the atom sites and the mean square displacements can be obtained. In this work, x-ray diﬀraction measurements

were performed at a Huber G670 diﬀractometer with copper Kα1 radiation in a Guinier geometry using an imaging plate detector and at the Advanced Photon Source, APS, with synchrotron radiation in Debye-Scherrer geometry using an imaging plate detector. The diﬀraction patterns were reﬁned by the Rietveld method using the FULLPROF36 program. The Gr¨uneisencoeﬃcient describes the dependence of the phonon mode frequency, ω(~k), to the volume of a unit cell, V : γ = −∂(ln ω(~k))/(∂(ln V )) and indicates the deviation of the lattice dynamics from the harmonic approximation, see below. The thermal conductivity is related to the anharmonicity and therefore the Gr¨uneisenparameter is a useful parameter in order to compare thermoelectric materials. From the temperature dependence of the lattice parameters, a(T ), the thermal expansion coeﬃcient, α, can be obtained by the derivative α = (da(T )/dT )/a(300K). The Gr¨uneisencoeﬃcient follows from the thermal expansion, the bulk modulus B, obtained e.g. by resonant ultrasound spectroscopy, the heat capacity

CV and the molar volume Vm: γ = 3αBVm/CV , see Chapter 2, 3 and 5.

VI. INELASTIC SCATTERING3,35,37

Inelastic scattering takes place, if there is an energy transfer between the scattered ra- diation and the probed object. Due to the energy transfer a creation or an annihilation of lattice vibrations, i.e. phonons, takes place. Inelastic scattering is thus a suitable method to study the lattice dynamics in materials. In this work, inelastic neutron scattering and nuclear inelastic scattering were used in order to investigate the lattice dynamics, and therefore to study the related thermal conductivity in thermoelectric Zintl phases. Phonons are quantized collective vibrations of atoms around their equilibrium positions in an atomic plane of a lattice. The amplitudes of these waves can be parallel, e.g. longitudinal, or perpendicular, e.g. transversal, to the phonon propagation wavevector ~k. In a simpliﬁed picture, the atoms in a plane are moving in phase in acoustic modes, whereas in optical modes the atoms are moving out of phase. A crystal with N atoms in the unit cell will have 3 acoustic modes, from which two are transversal and one is longitudinal, and (3N−3) optical phonon modes, from which 2/3 are transversal and 1/3 are longitudinal. The frequency of an Chapter 1: General Introduction – Inelastic Scattering 15

acoustic mode is zero at the Brillouin zone center, increases linearly in the long wavelength region, ~k π/a, and approaches a constant at the zone boundary, ~k = ±π/a, with the lattice parameter a. Optical modes have a non zero frequency at the zone center and the frequency is typically only slightly wavevector dependent. The dispersion relation gives the relation between the wavevector and the frequency of the phonon modes. The dispersion relation is dependent on the mass of the atoms and the force constants, i.e. the bonding of the atoms to each other. Furthermore, the dispersion is dependent on the wavevector direction in the Brillouin zone. In the Brillouin zone are special reciprocal lattice points of high symmetry and the typical presentation of phonon dispersions are between these points. The center of the Brillouin zone, ~k=(0,0,0), is denoted by Γ. For example, in a body centered cubic system, there are 3 directions to be consider from Γ towards the Brillouin zone boundaries at ~k=(1/2,0,0), labeled by X, at (1/2,1/2,0), labeled by M and at (1/2,1/2,1/2), labeled by R. The dispersion can be experimentally obtained by inelastic neutron scattering on a single crystal, see below and Chapter 4.

The density of phonon states, g(E), denotes the number of phonon modes in an energy interval. The density of phonon states is large, where the slope of the dispersion curve is small. If the slope of the dispersion curve is zero, the derivation with respect to the energy of the density of phonon states has a singularity, which is called Van Hove singularity. The total cross-section weighted density of phonon states can experimentally obtained by inelastic neutron scattering on a polycrystalline sample, see below and Chapter 3 and 5. The partial, e.g. element speciﬁc, density of phonon states can be obtained by nuclear inelastic scattering, see below and in Chapter 2, 3 and 5. From the density of phonon states, diﬀerent transport and thermodynamic properties can be deduced, see Chapter 2.

The occupation of the phonon states is temperature dependent and increases with tem- perature, as more modes get excited. The occupation number of the states, n(E), is given

by the Bose function: n(E) = 1/(1 − exp(E/(kBT ))), with the phonon energy E. For a harmonic crystal, this is the only temperature dependence of the density of phonon states. For a system with anharmonic eﬀects, e.g. thermal expansion, temperature dependence of the elastic constants or phase transitions, the harmonic approximation fails and the density of phonon states is temperature dependent after applying a correction of the Bose factor, see especially Chapter 4. Chapter 1: General Introduction – Inelastic Scattering 16

A. Inelastic Neutron Scattering38

In contrast to x-ray scattering by the electrons, the scattering process takes place between the nuclei and the neutron. Thermal neutrons have energies in the same order of magnitude as the excitation energy of phonons. Therefore, inelastic neutron scattering is a standard tool to measure the phonon dispersion and the density of phonon states. The elastic cross section for ~ 2 2 P ~ 2 coherent neutron scattering on the nucleus is dσ/dΩ = |F (Q)| = hbi | k exp(iQ~rk)| , with the scattering length b. The scattering length is not dependent on the number of electrons of the atom, as for x-rays, and neighboring atoms in the periodic table or even isotopes can have very diﬀerent scattering lengths. If the studied element has several isotopes or a non zero nuclear spin state, incoherent scattering can occur. In contrast to coherent scattering, the incoherent scattering cross section contains no phase information. Incoherent scattering depends only on the correlation between the positions of the same nucleus at diﬀerent times and shows therefore no interference eﬀects, whereas coherent scattering depends on the correlation between the positions of all nuclei at diﬀerent times and interference occurs.

In an inelastic neutron scattering process, the wavevector of the neutron is changed, ~ ~ |ki|= 6 |kf |, due to the energy transfer between the neutron and the probed sample. The momentum and the energy of the total system have to be conserved and accordingly the ~ ~ ~ ~ 2 ~ 2 ~ 2 following relations are obtained: Q = ki − kf = G + ~q and ~ω = (~/(2mn)) (ki − kf ), with the phonon wavevector ~q and the mass of a neutron mn. An inelastic scattering process is illustrated in Fig.8. The coherent part of the inelastic neutron cross section is dependent on the scattering vector Q~ , whereas the incoherent part scatters isotropically at all Q~ and is proportional to the density of phonon states for a cubic Bravais crystal. Some elements do not show signiﬁcant incoherent scattering. In order to determine a proper density of phonon states of coherent scatterer, the typical approximation is to average over a suﬃciently large Q~ range. In the incoherent approximation, the density of phonon states, g(E), can be directly obtained from the inelastic neutron scattering, S(E), by g(E) = S(E)E/n(E), with the Bose factor n(E), as described above.

There are essentially two types of inelastic neutron scattering instruments, the triple-axes spectrometers, typically used to study the phonon dispersion on a single crystal, and the time of ﬂight spectrometers, mostly used to study the density of phonon states on powders. Triple-axes spectrometer: The IN12 is a typical triple axis spectrometer, see Fig.9, and was Chapter 1: General Introduction – Inelastic Scattering 17

FIG. 8. An inelastic scattering process. ~q denotes the phonon wavevector. used in this work, see Chapter 4. The IN12 is located at the Institute Laue-Langevin (ILL) research reactor in Grenoble, France. The monochromator, the sample and the analyzer axis can be moved independently in order to cover a large range of energies and of wavevectors. After the neutron beam is monochromized by a single crystal monochromator, typically pyrolitic graphite, it hits the sample and is scattered. The scattered neutrons leave the sample and the analyzer selects neutrons at a deﬁned angle with given energy by Bragg scattering. Only neutrons with a given wavevector are scattered by the analyzer crystal towards the detector. In order to deﬁne the orientation of the crystal, a precharacterization measurement is necessary, e.g. by Laue diﬀraction. In order to obtain the phonon mode dispersion, an area around a Bragg reﬂection is scanned over a phonon wavevector and energy range. For measuring longitudinal modes, Q~ has to be parallel to ~q, for measuring transversal modes, Q~ has to be perpendicular to ~q. As an example, in order to obtain the acoustic longitudinal mode in [x,x,0] direction, a Q~ scan from (x, x, 0) to (x+1/2, x+1/2, 0) has to be carried out, in an energy range from 0 to ∼8 meV, see also Chapter 4. Time-of-ﬂight spectrometer: The velocity, v, of a neutron depends on its wavelength, λ, p and therefore on the energy of the neutron: v = h/(mnλ) = 2E/mn, with the mass of a neutron mn. This relation is used to analyze the scattered neutron energy in a time-of-ﬂight spectrometer. A sketch of a typical time-of-ﬂight spectrometer IN6 at the ILL, is shown in Fig.9. The neutron beam is monochromized by a crystal monochromator. The Fermi chopper deﬁnes the zero point of the neutron ﬂight path to the detector: Monochromatic neutron bunches with a ﬁxed time between each bunch hit the polycrystalline sample and are scattered elastically and inelastically. They will be scattered by the sample and will reach the detector in a time, depending of the energy of the neutron. If a neutron annihilates Chapter 1: General Introduction – Inelastic Scattering 18

FIG. 9. The triple-axes spectrometer IN12 (left) and the Time-of-Flight spectrometer IN6 (right) from Ref. [39].

a phonon, such that the energy of the neutron is increased, the neutron will reach the detector earlier, than an elastically scattered neutron. If the neutron creates a phonon, the neutron loose some energy and it will be slower than the elastically scattered neutrons. Since the distance between the Fermi chopper and the detector is well deﬁned, the energy of the scattered neutron can be determined. With this technique, the powder averaged Q~ dependence of the energy dependent scattering, S(Q, E), can be obtained. The scattering intensity typically shows a Q2 dependence in Q, due to the inelastic scattering cross section. By integrating over Q and multiplying with the Bose function, the total, neutron cross section weighted phonon density of states can be determined in the incoherent approximation, see Chapter 3 and 5. Further spectrometers used in this work are the cold neutrons time-of-ﬂight spectrometer FOCUS, Paul Scherrer Institut (PSI), Switzerland, and the wide angular range copper spectrometer, ARCS, at the Spallation Neutron Source (SNS), USA, which have similar setups, however, at ARCS the incident neutron energy is monochromized by Fermi choppers instead of a monochromator crystal. Chapter 1: General Introduction – Inelastic Scattering 19

B. Nuclear Inelastic Scattering40–42

This method is based on the M¨ossbauereﬀect. The M¨ossbauereﬀect describes the recoil- free absorption or emission of a γ-ray by a nucleus in a solid. When an excited nucleus de-excites by emitting a γ-ray typically the nucleus recoils to the opposite direction of the emitted γ-ray. The energy diﬀerence between the excited state and the ground state, E0, of a nucleus at rest is therefore divided into the emitted γ-ray energy Eγ and the recoil energy ER. The recoil energy is dependent on the mass of the nucleus and the γ-ray energy: 2 2 ER = Eγ /(2Mc ), with the speed of light c. The diﬀerence between the emitted and absorbed

γ-ray is 2ER and a resonant absorption process can only take place, if the natural width of the excited state, Γ, is a least twice of the recoil energy: Γ/2ER > 1. This condition is not fulﬁlled for free, unbound, atoms in a gas or liquid and therefore resonant absorption cannot take place in this case. However, if the excited nucleus is bound in a solid and de- excites, in a semi-classical picture the whole lattice will recoil and therefore the recoil energy is not dependent on the mass of the nucleus but on the mass of the whole crystal system.

Therefore, the recoil energy is small, Eγ ≈ E0, and resonant absorption can take place. 2 2 The Lamb-M¨ossbauerfactor describes the recoilless fraction fLM = exp(−k hu i), with the wavevector k of the emitted γ-ray and the mean-square displacement hu2i. If all atoms are

ﬁxed on their equilibrium positions, the fLM would be one. Due to lattice vibrations and zero point motions, the atoms moves and additional states exist between which the transition can take place, see ﬁgure 10. This lowers the fLM and by increasing temperature, more phonons are excited and fLM decreases. The fLM is analogous to the Debye-Waller factor in diﬀraction measurements.

Many M¨ossbauer isotopes can be studied by the NIS technique, but due to the limits of the available synchrotron radiation energy and adequate monochromators, isotopes with transition energies larger than ∼37 keV (121Sb) were not studied with NIS so far. Further- more, the lifetime of the excited state has to be long enough in order to separate nuclear ﬂuorescence and prompt scattering by an electronic detection veto, see below. Although it was shown that it is possible to measure NIS with the 201Hg resonance43, which exhibits a lifetime of 0.9 ns, no further measurements were carried out with this resonance so far. Therefore, 125Te can be regarded as the isotope with the shortest lifetime (1.5 ns) measurable by a standard NIS setup. At resonance energies above 40 keV, a further diﬃculty arises from Chapter 1: General Introduction – Inelastic Scattering 20

FIG. 10. An elastic nuclear resonant absorption process, solid line, and the incoherent inelastic

nuclear resonant scattering of a 1-phonon (dashed line) and a 2-phonon process (dotted line). E0

and Eph are the resonant transition energy and the phonon energy, respectively.

FIG. 11. Simpliﬁed setup for the measurement of the nuclear forward and the nuclear inelastic scattering from Ref. [44]. After the high-heat-load monochromator, HHLM, the photon energy bandwidth is in the eV region. The high-resolution monochromator, HRM, reduces the bandwidth to ∼1 meV and the beam is backscattered to the sample, S. The nuclear forward scattering de-

tector, DNFS, and the nuclear inelastic scattering detector, DNIS, detect the forward and inelastic scattering, respectivley.

2 2 the large recoil energy, ER = Eγ /(2Mc ), which leads to large multiphonon contributions. While the ﬁrst inelastic measurements were obtained in 1995 using the 57Fe resonance, the ﬁrst inelastic measurement on the newest isotopes were in 2006 and 2008 with the 121Sb resonance and with the 125Te resonance44, respectively. Since then tremendous increase in resolution has been achieved45 from ∼6 meV to now ∼1 meV. For this work, measurements with the 57Fe, 121Sb and 151Eu resonance were carried out, see Chapter 2, 3 and 5. The incoherent inelastic nuclear resonance scattering process is shown in Fig. 10. If the energy of the incident photon beam includes the transition energy of the nuclear resonance of the studied M¨ossbauerisotope, photons can be absorbed and the nucleus excites. After some Chapter 1: General Introduction – Inelastic Scattering 21 time, depending on the lifetime of the excited state and the hyperﬁne structure, the nucleus will decay to the ground state by emitting a photon with the same energy than the initial photon (nuclear forward scattering) or by nuclear ﬂuorescence. If the energy of the incident photon beam is slightly changed to a value near the transition energy, the photons can be absorbed only through simultaneous creation or annihilation of a phonon. Therefore, this method relies essentially on the phonon-assisted nuclear resonance absorption and can be used to directly probe phonon states. In order to measure the phonon spectrum the incident photon energy is tuned in an energy region of typically ±60 meV around the resonant transi- tion energy, while simultaneously the nuclear ﬂuorescence is detected. A typical spectrum is shown in Fig. 12. The instrumental setup is shown in Fig. 11, in this case for measurements at the 121Sb resonance with a Bragg backscattering monochromator. The synchrotron radiation bunches has to be well separated and the time between two bunches have to be long enough to measure the nuclear ﬂuorescence. After the high-heat-load monochromator, the energy of the photon beam has a bandwidth in the eV range. The high-resolution monochromator monochromizes this beam to a bandwidth of around ∼1 meV, which is the required reso- lution for measuring phonon modes. For measurements with the 57Fe and 151Eu resonance a nested monochromator41 was used, and for the 121Sb resonance a Bragg backscattering monochromator was used. The tuning of the energy of the latter monochromator is achieved by tuning the temperature of a high quality sapphire single crystal, on which the Bragg backscattering takes place: By tuning the temperature, the distance of the lattice planes changes due to thermal expansion, and therefore the wavelength of the photons, which fulﬁll Bragg’s law, is varied. The requested temperature tuning is in the mK region, see upper scale in Fig. 12, for more details see Ref. [44]. The photon beam hits the sample and the above described transitions can take place. An electronic veto has to be implied, in order to suppress the detection of the prompt Compton, Thomson and electronic ﬂuorescence scattering. The nuclear forward scattering, which is used to determine the instrumental res- olution, is detected in the forward scattering and the nuclear inelastic scattering is detected by the inelastic detector. Since nuclear ﬂuorescence is essentially isotropic in all directions, a large angular range has to be covered by the detector and the inelastic detector should be as close as possible to the sample. In order to obtain the density of phonon states from the spectrum, the instrumental resolution has to be taken into account and the one phonon term has to be extracted. After subtraction of the elastic line from the spectrum obtained Chapter 1: General Introduction – Inelastic Scattering 22

T-T0 (mK) 200 100 0 -100 -200 -300 150 K 16 40 K 80 14 12 60 10 8 40 6 Countrate NIS (Hz) 4 20 Countrate NFS (Hz) 2 0 0 -40 -20 0 20 40 60

E-E0 (meV)

FIG. 12. The nuclear inelastic scattering, NIS, measured on a polycrystalline elemental Sb sample with the 121Sb resonance at 40 K, blue, and 150 K, red, and the nuclear forward scattering, NFS, which was taken as the resolution function, black. The upper x label indicates the temperature change of the monochromator crystal corresponding to the energy transfer E − E0. The dotted lines indicate the multiphonon contribution at 40 K, blue, and 150 K, red. by the nuclear inelastic scattering detector, the spectrum has to be deconvoluted by the in- strumental resolution. Also, two or more phonon transitions can take place, see Fig. 10. The multiphonon contribution is dependent on the Lamb-M¨ossbauerfactor, fLM , and has to be subtracted from the spectrum. As described above, the Lamb-M¨ossbauerfactor is temper- ature dependent and decreases with temperature, see Fig. 12. For 57Fe, there is typically a much smaller decrease of the Lamb-M¨ossbauerfactor as for 121Sb. Therefore, Fe NIS can be measured at room temperature, but for 121Sb low temperature measurements are preferable, due to the large multiphonon contribution at high temperatures, and the therefore imprecise extraction of the one phonon term. From the extracted element speciﬁc density of phonon states the velocity of sound and the element speciﬁc Debye temperature, mean force constant and lattice heat capacity can be obtained42, see Chapter 2, 3 and 5. Chapter 1: General Introduction 23

1 D. M. Rowe, Thermoelectrics Handbook: Macro to Nano (Taylor & Francis Group, Boca Raton, 2006). 2 B. C. Sales, Science 295, 1248-1249 (2002). 3 N. W. Ashcroft, and N. D. Mermin, Solid State Physics (Thomson Learning, 1976). 4 H. J. Goldsmid, Introduction to Thermoelectricity (Springer-Verlag Berlin Heidelberg, 2010). 5 G.A. Slack, CRC ’Handbook of Thermoelectrics’, 407-440 (CRC Press, 1995). 6 J. R. Sootsman, D. J. Chung, and M. G. Kanatzidis, Angew. Chem. Int. Ed. 48, 8616-8639 (2009). 7 D. M. Rowe, Modern Thermoelectrics, (Holt, Rinehart and Winston Ltd., 1983). 8 N. Wiberg, Lehrbuch der Anorganischen Chemie (de Gruyter, Berlin, 1995). 9 E. S. Toberer et al., Chem. Mater. 22, 624-634 (2010). 10 S. M. Kauzlarich S. R. Brown, and G. J. Snyder, Dalton Trans. 21, 2099-2107 (2007). 11 J. Y. Chan et al., Chem. Mater. 10, 3583-3588 (1998). 12 B.C. Sales et al., Science 272, 1325-1328 (1996). 13 G. S. Nolas et al., J. Appl. Phys. 79, 4002-4008 (1996). 14 G. S. Nolas, J. L. Cohn, and G. A. Slack, Phys. Rev. B 58, 164-170 (1998). 15 D. T. Morelli et al., Phys. Rev. B 56, 7376 (1997). 16 B. C. Sales et al., Phys. Rev. B 56, 15081-15089 (1997). 17 M. Christensen et al., Nature Materials 7, 811-815 (2008). 18 M. M. Koza et al., Nature Materials 7, 805-810 (2008). 19 N. R. Dilley et al., Phys. Rev. B 61, 4608-4614 (2000). 20 M. D. Hornbostel et al., J. Am. Chem. Soc. 119, 2665-2668 (1997). 21 M. Beekman et al., J. Phys.: Condens. Matter 22, 355401 (2010). 22 J. Dong, O. F. Sankey, and C. W. Myles, Phys. Rev. L 86, 2361-2364 (2001). 23 G. S. Nolas et al., Appl. Phys. Lett. 82, 910-912 (2003). 24 R. P. Hermann et al., Phys. Rev. B 72, 174301 (2005). 25 B. C. Sales et al., Phys. Rev. B 63, 245113 (2001). 26 L. Qiu et al., Phys. Rev. B 70, 035208 (2004). 27 S. R. Brown et al., Chem. Mater. 18, 1873-1877 (2006). Chapter 1: General Introduction 24

28 G.A. Slack, Solid State Physics 34, edited by H. Ehrenreich, 1-71 (Academic Press, 1979). 29 Manual to the Physical Properties Measurement System (PPMS) from Quantum Design. 30 A. Migliori et al., PHYSICA B 183, 1-24 (1993), and A. Migliori, and J. L. Sarrao, Resonant ultrasound spectroscopy (Wiley, New York, 1997). 31 L. Zhang et al., Mater. Sci. Eng. B 170, 26-31 (2010). 32 Y. P. Varshni, Phys. Rev. B 2, 3952-3958 (1970). 33 V. Keppens et al., Nature 395, 876-878 (1998). 34 R. B. Schwarz, and J. F. Vuorinen, J. Alloys Comp. 310, 243-250 (2000). 35 C. Kittel, Einf¨uhrungin die Festk¨orperphysik (R. Oldenbourg Verlag GmbH, M¨unchen, 1996). 36 J. Rodriguez-Carvajal, FULLPROF V (2009)(Laboratoire Leon Brillouin (CEA-CNRS), France, 2009). 37 M. T. Dove, Introduction to Lattice Dynamics (Cambridge University Press, 1993). 38 G.L. Squires, Introduction to the theory of thermal neutron scattering, (Cambridge University Press, 1978). 39 http://www.ill.eu/ﬁleadmin/users ﬁles/Other Sites/YellowBook2008CDRom/index.htm 40 Y.-L. Chen, and D.-P. Yang, M¨ossbauer Eﬀect in Lattice Dynamics (WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim, 2007). 41 R. R¨ohlsberger, Nuclear Condensed Matter Physics with Synchrotron Radiation, (Springer- Verlag Berlin Heidelberg, 2004). 42 R. R¨uﬀer,and A. I. Chumakov, Hyp. Interact. 128, 225-272 (2000). 43 D. Ishikawa, A. Q. R. Baron, and T. Ishikawa, Phys. Rev. B 72, 140301(R) (2005). 44 H. C. Wille et al., Europhys. Lett. 91, 62001 (2010). 45 I. Sergueev et al., J. Synch. Rad., submitted (2011). Chapter 2

Lattice Dynamics in the FeSb3 Skutterudite

25 Lattice Dynamics in the FeSb3 Skutterudite

A. M¨ochel,1, 2 I. Sergueev,3 N. Nguyen,4 Gary J. Long,5 F. Grandjean,2 D. C. Johnson,4 and R. P. Hermann1, 2, ∗

1J¨ulichCentre for Neutron Science JCNS and Peter Gr¨unberg Institut PGI, JARA-FIT, Forschungszentrum J¨ulichGmbH, D-52425 J¨ulich,Germany 2Facult´edes Sciences, Universit´ede Li`ege,B-4000 Li`ege,Belgium 3European Synchrotron Radiation Facility, F-38043 Grenoble Cedex, France 4Department of Chemistry and Materials Science Institute, University of Oregon, Eugene, OR 97403, USA 5Department of Chemistry, Missouri University of Science and Technology, University of Missouri, Rolla, Missouri 65409-0010, USA

Abstract

Thin ﬁlms of FeSb3 were characterized by electronic transport, magnetometry, x-ray diﬀrac- tion, 57Fe and 121Sb nuclear inelastic scattering, and 57Fe M¨ossbauerspectroscopy. Resistivity and magnetometry measurements reveal semiconducting behavior with a 16.3(4) meV band gap and an eﬀective paramagnetic moment of 0.57(6) µB, respectively. A systematic comparison of the lat- tice dynamics with CoSb3 and EuFe4Sb12 reveals that the [Fe4Sb12] framework is softer than the

[Co4Sb12] framework, and that the observed softening and the associated lowering of the lattice thermal conductivity in the RFe4Sb12 ﬁlled skutterudites is not only related to the ﬁller but also to the [Fe4Sb12] framework.

PACS numbers: 63.20.D-, 76.80.+y, 72.20.Pa, 61.05.C-, 65.40.Ba, 65.40.De,

26 Chapter 2: FeSb3 – Introduction 27

I. INTRODUCTION

Skutterudites are promising thermoelectric materials that have been intensively stud- ied since the 1990s1–4. They possess interesting semiconducting properties, notably a large Seebeck coeﬃcient, and a relatively low thermal conductivity that has been ascribed to the dynamics of the ﬁller5–7. In particular the lattice dynamics of ﬁlled and unﬁlled skut- terudites has been the object of intensive research8–12. The semiconducting, magnetic, and 6,13 thermal properties of the ﬁlled R(Fe,Co)4Sb12 skutterudites can be tuned by ﬁlling the + + 2+ (Fe,Co)4Sb12 framework with monovalent ions, e.g. Na and Tl , divalent ions, e.g. Yb and Eu2+, or trivalent ions, e.g. La3+ and Ce3+. However, only a limited degree of ﬁlling 6,13,14 can be achieved in CoSb3. In order to achieve larger degrees of ﬁlling either Co must be substituted by Fe or a synthesis involving ball milling and subsequent hot pressing must be used15.

Because there is no bulk synthesis procedure, the inﬂuence of ﬁlling the FeSb3 structure on its lattice dynamics has been studied by diﬀerent approaches. The direct comparison with the lattice dynamics of the [Fe4Sb12] polyanion is not possible, thus one approach is the comparison9,10 of the lattice dynamics of the ﬁlled structures mentioned above with the related unﬁlled CoSb3. Another approach is the study of the contribution of the ﬁller R to the density of phonon states (DPS). Density functional theory calculations of the partial density of phonon states have been carried out and compared with experimental data, obtained by inelastic neutron scattering and nuclear inelastic scattering16,17. The partial contributions to the DPS can also be investigated by ab initio powder-averaged lattice dynamic calculations and a subsequent comparison with inelastic neutron scattering measurements11.

18,19 The synthesis of FeSb3 is however possible by nanoalloying and this approach has recently been improved and now yields higher sample purity, but still produces only small amounts in the form of micrometer thick ﬁlms. Because detailed knowledge of the lattice dynamics in skutterudites is necessary to unravel the mechanisms that yield their low thermal conductivity, characterization methods suitable for thin ﬁlms have to be used. Although inelastic neutron scattering experiments are in principle feasible, the beamtime required would be prohibitively long because of the small amount of sample. In contrast, nuclear inelastic scattering (NIS) is a method of choice that yields the DPS for selected elements20 even with small samples. This method has been applied21 to the 57Fe nuclear resonance for Chapter 2: FeSb3 – Experimental 28 some time, and has recently been developed17 for the 121Sb resonance. The resolution for the latter isotope was recently improved22 to ∼1.3 meV full width at half maximum (FWHM).

It is thus possible to fully access the element speciﬁc DPS in FeSb3 and to obtain several related quantities20, such as the mean force constants, the atomic displacement parameters, and the average velocity of sound.

Herein we report both the macroscopic characterization of high purity FeSb3 by resis- tivity and susceptibility measurements and the microscopic characterization by synchrotron radiation diﬀraction, 57Fe M¨ossbauerspectral measurements, and nuclear inelastic scattering 57 121 by Fe and Sb. A comparison of these results with the properties of CoSb3 reveals that

FeSb3 is signiﬁcantly softer, an observation that both reveals a combined inﬂuence of the ﬁller and the substitution of Fe for Co on the lattice dynamics and hence thermal properties, and provides additional clues to the low thermal conductivity in ﬁlled skutterudites.

II. EXPERIMENTAL

The FeSb3 thin ﬁlms were deposited on Kapton foil at ambient temperature by the elemental modulated reactant method in a custom-built ultra high vacuum, ≈ 10−5 Pa, deposition system described elsewhere23. Fe was deposited by using a 3 kW electron beam gun at a rate of 0.4 A/s˚ and Sb was deposited by using an eﬀusion cell at a rate of 0.6 A/s.˚ A computer was used to control the deposition procedure. A quartz crystal monitoring system placed 25 cm above each source was used to control the elemental layer modulation, the deposition rates, the shutter opening time for Fe, and the thickness for Sb. The precursors for the crystallized ﬁlms were prepared by depositing multiple alternate layers of Fe and Sb until the desired ﬁlm thickness was obtained. Deposition parameters were determined to yield the appropriate molar stoichiometry of FeSb3. These precursor ﬁlms were then annealed under a nitrogen atmosphere at 410 K to form FeSb3. With this method, two ﬁlms of thicknesses of ∼1 and ∼1.5 µm were deposited on a 25 µm thick Kapton substrate. All further measurements were carried out on these two ﬁlms. Temperature dependent resistivity and magnetization measurements were carried out between 10 and 300 K on a physical properties measurement system (QD-PPMS) with the resistivity and the vibrating sample magnetometer option. The resistivity was measured on several 1 µm thick samples with 2 by 5 mm2 lateral dimension with diﬀerent microcrack Chapter 2: FeSb3 – Experimental 29

structures, see below. The magnetization measurements were carried out with an applied magnetic induction of 0.25 T on a 80 cm by 3.7 mm long wrapped ribbon of the 1 µm thick

ﬁlm, i.e. ∼12.9 mg of FeSb3. Hysteresis measurements have been carried out at 300 K up to 1.5 T in order to assess the presence of impurity phases and the diamagnetic contribution to the susceptibility. The same measurements have been carried out on polycrystalline CoSb3 for comparison. The susceptibility, χ, was calculated from the magnetization by assuming the validity of the low ﬁeld limit approximation χ = M/H, where M is the magnetization and H the applied ﬁeld.

Temperature dependent x-ray diﬀraction measurements were carried out at the 6-ID- D high-energy station at the APS between 10 and 300 K. The x-ray wavelength was 0.124269 nm, the area detector was at 1601 mm from the sample, and silicon (Chempur, 99.999%) was used as an internal standard. The sample contained 10 layers of a ∼1.5 µm thick ﬁlm of FeSb3 on Kapton foil and, for better thermal coupling to the sample holder, Al foil was placed between each layer. The powder diﬀraction pattern of CoSb3 was measured under the same conditions. The data was reduced to diﬀractograms by using Fit2D24 and analyzed using the Rietveld method25.

The 57Fe M¨ossbauer spectra have been measured between 4.2 and 295 K on a constant- acceleration spectrometer that utilized a 295 K rhodium matrix 57Co source and was cali- brated at 295 K with α-Fe powder.

121 The Sb NIS by FeSb3 was measured at the ID22N station at the ESRF operating in 16- bunch mode. A resolution of 1.3 meV was reached by using a high resolution backscattering monochromator with the (8 16 24 40) reﬂection of a sapphire single crystal cooled to ∼237 K.

The sample containing 6 layers of a ∼1.5 µm thick ﬁlm of FeSb3 on Kapton foil with Al foil between each layer was cooled to 25 K in order to minimize multiphonon scattering. The 121 Sb NIS of CoSb3 and EuFe4Sb12 was measured on powder samples with the same setup 57 and resolution. The 295 K Fe NIS on the same FeSb3 sample was measured at the ID18 station at the ESRF operating in 16 bunch mode with a resolution of 0.7 meV. Chapter 2: FeSb3 – Electric transport and magnetism 30

FIG. 1. The structure of unﬁlled CoSb3 or FeSb3 (left) and ﬁlled RFe4Sb12 (right) skutterudite. Co or Fe, Sb, and R are shown in red, blue, and yellow, respectively. The blue rectangle indicates one of the Sb rings, see text.

III. RESULTS AND DISCUSSION

A. Electric transport and magnetism

Above ∼40 K the electrical resistivity, ρel, of FeSb3 decreases with increasing temperature, see Fig.2, a decrease that is indicative of semiconducting behavior. A ﬁt of the data in high 26 temperature region, see upper inset in Fig.2, with ρel(T ) = A · exp(Eg/2kBT ), where Eg is the energy gap, kB the Boltzmann constant, T the temperature, and A a proportionality constant, yields an electronic band gap of 16.3(4) meV, a narrower gap than the 50 meV gap 26 obtained by resistivity measurements on lightly p-doped CoSb3. As expected for rather thin ﬁlms, the microstructure was found to be very important and resistivity measurements were carried out on several samples. The smallest cracks or scratches will increase the resistivity by several orders of magnitude with respect to pristine samples, see the lower inset in Fig.2. Further, heating the sample above 300 K, not shown, induces additional microstructure and increases the resistivity, because of the diﬀerential thermal expansion between Kapton and

FeSb3. Atomic force microscopy measurements were carried out to monitor this behavior and to assure that the results in Fig.2 were obtained on a sample free of cracks at the ∼50 nm level. Such a dependence of the resistivity on the microstructure has also been 27 observed in polycrystalline CoSb3, with reported resistivities of undoped samples between Chapter 2: FeSb3 – Electric transport and magnetism 31

FIG. 2. Electrical resistivity, ρel, of FeSb3 obtained between 10 and 300 K on a crack free sample, the errors are the size of the data points. The lower left inset shows a comparison between 10 and 150 K of the crack free (red) and a cracked sample (green) on a logarithmic scale. The top right inset shows the ﬁt between 220 and 300 K, see text. The top left shows an atomic force microscopy depth contrast view of a cracked sample.

7 and 1000 µΩm at room temperature27–33. The 300 K resistivity of 29.4(1) µΩm observed 30 for crack free FeSb3 is similar to the 37 µΩm of a polycrystalline, sintered, CoSb3 sample , which also exhibits the temperature dependence of a typical semiconductor.

The molar susceptibilities, χm, of FeSb3 and CoSb3 are shown in Fig.3. First, the diamag- netic contribution was obtained from the slope of a hysteresis loop measurement at 300 K, see Fig.4, and is associated with the sample holder, the ion core diamagnetism, and, for dia the FeSb3 ﬁlms, to the Kapton substrate. The resulting corrections of χm were assumed to be temperature independent and were used to obtain the results shown in Fig.3. Second, the ferromagnetic contribution resulting from a small amount of ferromagnetic impurity in

FeSb3 was obtained from the hysteresis loop, see Fig.4, and corrected for. The magnetiza- tion of this impurity is essentially saturated at 0.25 T. Finally, a small correction term, χ0, amounting to ∼12% of the diamagnetic correction was added to account for imperfections in the correction procedure. Adding this χ0 immediately yielded paramagnetic Curie-Weiss behavior for FeSb3 between 70 and 300 K. A plot of 1/χm, see left inset in Fig.3, yields Chapter 2: FeSb3 – Electric transport and magnetism 32

3.0 FeSb3 CoSb3 2.5 6e+08 0.60 ) 3 -8 2.0 4e+08 0.55 /f.u.) B 10 µ (mol/m ( x m

2e+08 eff 0.50 χ µ 1.5 1/

/mol) 0 0.45 3 0 100 200 300 0 100 200 300 (m

m 1.0 χ

0.5

0.0 0 50 100 150 200 250 300 T (K)

FIG. 3. The molar magnetic susceptibility obtained at 0.25 T between 10 and 300 K for FeSb3

(red) and CoSb3 (blue) after subtraction of both the diamagnetic contribution, calculated from the slope of a hysteresis loop at 300 K shown in Fig.4, and the ferromagnetic contribution. The errors are the size of the data points. Left inset: the inverse susceptibility of FeSb3. Right inset:

the eﬀective moment of FeSb3.

a Curie constant of 0.0414(1) m3K/mol with a 0 K Curie-Weiss temperature. The right

inset of Fig.3 indicates, that the eﬀective paramagnetic moment of FeSb 3 of 0.57(6) µB √ per formula unit, obtained from µeff = 797.8 · χm · T , is temperature independent above

∼70 K. The same approach was used for CoSb3 and an eﬀective paramagnetic moment of 33 0.10(6) µB/f.u. was obtained, a value that is compatible with an earlier report . A study

of Co1−xFexSb3 with x ranging from 0 to 0.1 has shown, that µeff increases with increasing 32 Fe content up to a maximum of 1.7 µB/f.u., a value that could correspond to low spin 3+ Fe . This behavior obviously does not extrapolate to FeSb3, which exhibits a much smaller eﬀective paramagnetic moment. From the y axis intercept of the magnetic hysteresis loop in Fig.4 an impurity phase of

0.004(1) atom % was obtained by assuming a typical mean value of 2.2 µB per Fe impurity atom at room temperature. The coercive ﬁeld of ∼80 Oe indicates, that the impurity phase

is not elemental Fe. For CoSb3 an elemental Co impurity phase of 0.0005(2) atom % was obtained by the same procedure. Chapter 2: FeSb3 – X-ray diﬀraction 33

0.003

0.002

0.001 /f.u.)

B 0.000 0.0003 µ (

M -0.001 0.0000 -0.002

-0.003 -0.0003 -0.3 0.0 0.3 -1.5 -1.0 -0.5 0.0 0.5 1.0 1.5 µ 0H (T)

FIG. 4. Hysteresis loop of FeSb3 measured at 300 K. The negative slope is indicative of diamagnetic behavior. The inset shows the hysteresis loop obtained after the diamagnetic correction discussed in the text.

B. X-ray diﬀraction

18,34 X-ray diﬀraction, see Fig.5, indicates , that both FeSb3 and CoSb3 form a cubic lattice with space group Im3 (number 204) and have the skutterudite structure, see Fig.1, where Fe or Co and Sb are located on the 8c and 24g sites, respectively. The inset to Fig.5 shows the detector image with homogeneous Debye-Scherrer rings that indicate the absence of texture. Apart from the Si internal standard no reﬂections from a secondary phase or the Al thermalization layers are observed. Because of the large background resulting from the 10 layers of Kapton foil, the Fourier ﬁltering option was used to properly subtract the background. The parameters obtained at 10 and 300 K by Rietveld reﬁnements are given in TableI. The Sb occupation was reﬁned assuming full occupation of the Fe or Co site. The density obtained from the lattice parameters is also given in TableI. A temperature dependent diﬀraction study on CoSb3 was carried out for comparison and the reﬁnement parameters given in TableI are in good agreement with the literature values 34. From the reﬁnement of the Sb occupation at 10 K a stoichiometry of FeSb2.88(5) and CoSb2.97(5) has been obtained. The corresponding 0.96(1) Sb occupancy in FeSb3 is however questionable, Chapter 2: FeSb3 – X-ray diﬀraction 34

see discussion in the M¨ossbauerspectroscopy part below.

A study of the Co1−xFexSb3 solid solutions, with x between 0 and 0.1, reveals that their lattice parameters increase linearly with increasing Fe content, in agreement with Vegard’s law32. If we assume, that this linearity holds true for higher Fe content, a lattice parameter of 9.126 A˚ is expected for FeSb3, a value that is in clear disagreement with the much larger 9.2383(3) A˚ found herein at 300 K. The thermal expansion calculated from the temperature dependence of the lattice parameters is shown in Fig.6. In order to reduce noise in this data, especially at low temperatures, the temperature dependence

of the lattice parameters was ﬁrst modeled with a third-order polynomial function, am(T ), see the ﬁt lines in the top of Fig.6. The diﬀerences between the ﬁtted curve and the data was less than 4 · 10−4 A.˚ The thermal expansion coeﬃcient, α, was then obtained from the derivative α = (dam(T )/dT )/am(300K). The thermal expansion coeﬃcient of CoSb3 at 220 K, 8.8·10−6 K−1, is in good agreement with the literature value35 of 9.1·10−6 K−1 as obtained from dilatometry. The thermal expansion of FeSb3 is larger as compared with

CoSb3. Under the assumption, that Poisson’s ratio for CoSb3 [9], ν = 0.22, is the same for 36 FeSb3, the bulk modulus can be extracted from the sound velocity , which can be obtained 37 from NIS, see below. The Gr¨uneisencoeﬃcient , γ = 3αBVm/CV , can be obtained by using the thermal expansion coeﬃcient, the bulk modulus, B = 47.9(1) and 83.2(1) GPa for FeSb3 and CoSb3, respectively, the molar volume, Vm, and the heat capacity, CV , see below. In

FeSb3 the resulting γ value of 1.4(1) at 300 K is only slightly larger than the 1.30(5) obtained for CoSb3, because FeSb3 exhibits at the same time a much larger thermal expansion and a much smaller bulk modulus compared to CoSb3.

2 The reﬁned isotropic mean square displacements, hu i, for Fe and Sb in FeSb3 are shown 38 2 2 2 in Fig.7. From the slope of the mean square displacements , dhu i/dT = 3~ /(mkBθD), where m is the mass of Sb or Fe, ﬁtted between 100 and 300 K, Debye temperatures, θD, of 230(5) and 410(10) K for Sb and Fe, respectively, have been obtained. The average value of av the Debye temperature in FeSb3, calculated from θD = (3θD,Sb + θD,Fe/Co)/4, is 275(5) K.

The mean square displacements of Sb and Co in CoSb3 are also shown in Fig.7. In CoSb 3 the Debye temperatures of 280(10) and 380(30) K for Sb and Co, respectively, have been av obtained, and θD = 305(15) K is larger than in FeSb3; the average value is in good agreement 39 with the literature value of 307 K, obtained by heat capacity, for CoSb3. Sb is located on a general (0, y, z) position and the y and z positions have been reﬁned. Chapter 2: FeSb3 – X-ray diﬀraction 35

FIG. 5. X-ray diﬀraction pattern of FeSb3 obtained at 10 K, red dots, the corresponding Rietveld reﬁnement, black line, the diﬀerence plot, blue line, and the peak positions for FeSb3 and Si, green ticks. Inset: a quarter of the corresponding detector image.

TABLE I. Rietveld reﬁnement parameters for FeSb3 and CoSb3. * constrained to the 10 K value.

FeSb3 FeSb3 CoSb3 (10 K) (300 K) (300 K)

Bragg R-factor (%) 7 6 6

Rf (%) 6.5 6.5 5 a (A)˚ 9.2116(3) 9.2383(3) 9.0320(5) y Sb 0.3402(2) 0.3399(3) 0.3356(3) z Sb 0.1578(2) 0.1573(3) 0.1586(3) Sb occupation 0.96(1) 0.96(1)* 0.99(1) Density (g/cm3) 7.157(1) 7.096(1) 7.648(1) Chapter 2: FeSb3 – M¨ossbauerspectroscopy 36

9.24 9.05 FeSb3 CoSb3 9.23 fit FeSb3 9.04 fit CoSb3 ] (Å) ] (Å) 3 3 9.22 9.03 [FeSb [CoSb a 9.21 9.02 a

9.20 9.01 14 14.0 /K] −6 12 12.0

/K) 10 10.0 −6 8 8.0 (10 α 6 6.0 4 FeSb3 4.0 CoSb3 2 2.0 thermal expansion [10 0 100 200 300 T (K)

FIG. 6. The temperature dependence of the lattice parameter, a, for FeSb3, in red, and CoSb3, in green, and the corresponding polynomial ﬁt, top. The thermal expansion coeﬃcient, α, of FeSb3 and CoSb3, bottom.

The sum y + z is 0.4972(6) and 0.4942(6) for FeSb3 and CoSb3, respectively. FeSb3 more closely fulﬁlls the Oftedal relation40, y + z = 1/2, which indicates that the rectangular Sb rings, see Fig.1, are closer to squares in FeSb 3 than in CoSb3.

C. M¨ossbauerspectroscopy

57 The 4.2 and 295 K Fe M¨ossbauerspectra of the ∼1.5 µm ﬁlm of FeSb3 are shown in the upper panel of Fig.8; the spectra obtained for both ﬁlms and at intermediate temperatures are very similar. In addition to the diﬀraction measurements, that revealed no crystalline impurity phase, no further amorphous iron bearing impurity is observed. All measured spec- tra were ﬁtted with a simple symmetric quadrupole doublet with two Lorentzian lineshapes, whose parameters are given in TableII. The M¨ossbauerspectra show no evidence for a second component related to Fe with missing Sb near neighbors, as would be expected from Chapter 2: FeSb3 – M¨ossbauerspectroscopy 37

0.03

FeSb3 Sb FeSb3 Fe ) 2 0.02 CoSb3 Sb CoSb3 Co

> (Å FeSb Sb (NIS)

2 3 u FeSb3 Fe (NIS) < 0.01

0.00 0 50 100 150 200 250 300 T (K)

FIG. 7. The mean square displacements, hu2i, obtained from the temperature dependent x-ray diﬀraction by FeSb3 and CoSb3 and NIS for FeSb3, see below. the hypothetical partial Sb occupancy seen in the diﬀraction measurements. The 96(1)% Sb occupancy, see TableI, would imply that more than 20% of the Fe have less than 6 Sb near neighbors, which would be visible in the M¨ossbauerspectra. The temperature dependence of the isomer shift, δ, quadrupole splitting, ∆EQ, linewidth, Γ, and the recoil-free fraction, fLM , is shown in the lower portion of Fig.8. The temperature dependence of δ and fLM have been ﬁt with a Debye model for a solid41.

The temperature dependence of the isomer shift is well ﬁt with the Debye model42 for the second-order Doppler shift with a characteristic M¨ossbauertemperature, θM , of 541(10) and 530(10) K for the ∼1.5 and ∼1 µm ﬁlms, respectively. This temperature is much larger than the Debye temperature, θD,Fe, of 350(5) and 373(6) K of the ∼1.5 and ∼1 µm ﬁlms, respectively, obtained from the temperature dependence of the logarithm of the spectral absorption area, fLM . The latter values are in good agreement with the values obtained 42 herein by other techniques, see TableIII. It is known that the two temperatures, θM and θD,Fe, obtained from the two temperature dependencies are usually diﬀerent because they depend, for the isomer shift, on hv2i, the mean-square vibrational velocity of the 57Fe, Chapter 2: FeSb3 – M¨ossbauerspectroscopy 38

100 295 K 99

98

97

4.2 K 96

Transmission, % 95

94

93 a)

-3 -2 -1 0 1 2 3 Velocity (mm/s) 0.5 1.0 δ b) δg(E) SOD 0.9

fLM (mm/s) δ 0.4 0.8 LM f , and Q

E ∆ EQ

∆ 0.7 , Γ

0.3 Γ 0.6 0 100 200 300 Temperature, K

FIG. 8. Upper panel: The M¨ossbauerspectra of FeSb3 obtained on a 1.5 µm ﬁlm. Lower panel: The ﬁt parameters obtained from the spectra of the ∼1 and ∼1.5 µm ﬁlms, open and closed symbols, respectively. The errors are the size of the symbols. The crossed square indicates the fLM obtained directly from the 57Fe NIS at 295 K. The dashed line indicates the second order Doppler shift

41 obtained from the DPS, see text. The lines for the Doppler shift and fLM are Debye model ﬁts .

The lines for ∆EQ and Γ are quadratic polynomial ﬁts given as guide to the eye. Chapter 2: FeSb3 – Nuclear resonance scattering 39 and, for the absorption area, on hu2i, the mean-square atomic displacement of the 57Fe; there is no model independent relationship between these mean square values42. However, 43 measurements of the M¨ossbauertemperatures on various compounds indicate that θM is often twice as large as θD,Fe, i.e. the isomer shift is more sensitive to higher energy phonons.

The Fe DPS of FeSb3, see below, clearly reveals that the Fe vibrations have a strong non- Debye behavior and are dominated by two strong optical modes above 30 meV. Because we have measured the partial DPS, g(E), by 57Fe NIS, see below, we can directly obtain the 42 g(E) 2 20 second order Doppler shift δSOD = −hv i/(2c) from the average kinetic energy hEkini = ∞ 2 R 1/2mRhv i = 3/4 coth(E/(2kBT ))g(E)EdE, where mR is the mass of the resonant nucleus. 0 The obtained temperature dependence of the isomer shift with the second order Doppler correction is shown in Fig.8, and corresponds to θM = 440 K. The diﬀerence is thus only partly explained and other corrections such as thermal expansion, which modiﬁes the DPS and therefore hEkini, or the inﬂuence of charge carrier activation on the isomer shift might be necessary.

D. Nuclear resonance scattering

121 The nuclear inelastic scattering spectra from the Sb NIS measurements in FeSb3,

CoSb3, and EuFe4Sb12 are shown in Fig.9, together with the instrumental functions mea- sured by nuclear forward scattering. The resolution of the instrument was ∼1.3 meV for all measurements. 121Sb NIS measurements on the latter two compounds have been published previously17 with a resolution of 4.5 meV. The measurements have been repeated, because of the enhanced resolution22. After subtraction of the elastic peak, the extraction of the DPS has been performed by the conventional procedure21,44, i.e. the correction of the mul- tiphonon contribution of the Fourier transformation of the inelastic scattering, which was slightly modiﬁed in order to take into account the asymmetry of the instrumental function; the data were deconvoluted by the experimental instrumental function and convoluted with a symmetric Gaussian with a FWHM of 1.7 meV, a value slightly larger than the ∼1.3 meV resolution that was chosen in order to avoid unphysical termination ripples in the DPS. The validity of the procedure was conﬁrmed by applying the usual sum rules45. The 57Fe NIS spectrum of FeSb3 measured at 295 K is also shown in Fig.9. The instrumental resolution was 0.7 meV and the DPS was obtained by the conventional procedure44. After the mul- Chapter 2: FeSb3 – Nuclear resonance scattering 40

TABLE II. M¨ossbauerspectral parameters for the FeSb3 ﬁlms. The errors are estimated to be 0.005 mm/s for the isomer shift, δ, quadrupole splitting, ∆EQ, and linewidth, Γ, and 0.005 (%)(mm/s) for the absorption area. aThe isomer shifts are given relative to 295 K α-Fe powder.

Thickness T δ ∆EQ Γ Total Area (µm) (K) (mm/s)a (mm/s) (mm/s) (%) (mm/s)

1 295 0.390 0.338 0.297 1.668 225 0.432 0.350 0.302 1.798 155 0.463 0.363 0.307 1.917 85 0.490 0.373 0.309 2.029 60 0.491 0.379 0.306 2.037 30 0.494 0.375 0.306 2.040 4.2 0.493 0.375 0.315 2.070 1.5 295 0.389 0.333 0.276 2.808 225 0.432 0.347 0.293 3.045 155 0.465 0.366 0.309 3.266 85 0.490 0.373 0.312 3.471 60 0.489 0.375 0.303 3.526 30 0.490 0.373 0.312 3.577 4.2 0.493 0.375 0.312 3.564

tiphonon correction, the partial DPS, g(E), were obtained, see Fig. 10, which also shows 57 the Fe DPS of EuFe4Sb12 from Ref. 46. The Fe DPS consists of two small broad peaks at ∼7 and 15 meV and a large broad peak around 30 meV. The latter broad peak is split and corresponds to a somewhat softer phonon mode in the EuFe4Sb12 ﬁlled skutterudite.

The splitting of this peak was also observed in the ﬁlled skutterudite LaFe4Sb12 by inelastic 16 46 neutron scattering measurements , and in CeFe4Sb12 by NIS . The low energy portion of the DPS indicates that FeSb3 is softer than EuFe4Sb12 as seen from the large increase in the reduced DPS, g(E)/E2, see insets to Fig. 10. The Sb vibrations mainly appear below 25 meV, but a small contribution of the Sb vibrations is also observed around 30 meV. The Chapter 2: FeSb3 – Nuclear resonance scattering 41 latter part of the DPS is not well resolved due to the multiphonon contributions in the ex- perimental data. By comparing the partial DPS in diﬀerent compounds, we observe that the

Sb DPS in CoSb3 exhibits pronounced features such as gaps at 12 and 21 meV and a well resolved peak at 23 meV. Inelastic neutron scattering measurements have also revealed16 this better resolution of the individual peaks in CoSb3 as compared with RFe4Sb12. How- ever, this diﬀerence is not directly related to the ﬁlling of the skutterudites, because the

DPS of FeSb3 shows the same broad features as EuFe4Sb12. The most pronounced diﬀerence of the DPS in FeSb3 as compared to other ﬁlled and unﬁlled skutterudites is an overall softening of the phonon modes, which leads to an enhancement of the DPS between 5 and

10 meV. This softening, which is also observed in the Fe DPS in FeSb3 at low energies, see Fig. 10, indicates a lower velocity of sound and might be crucial in determining the thermal conductivity and therefore the thermoelectric properties of skutterudites. In EuFe4Sb12 the essentially single frequency and Einstein like DPS of the Eu ﬁller appears46 at ∼7 meV. The relative hardening of the Sb DPS between FeSb3 and EuFe4Sb12, seen in the lower DPS of

EuFe4Sb12 at ∼7 meV, might be related to the appearance of this ﬁller mode. Calculations of the lattice dynamics in FeSb3 would thus be highly desirable in order to conﬁrm this hypothesis.

Several thermodynamic and vibrational quantities can be obtained from the DPS20. The element speciﬁc heat capacity, CV , can be directly calculated from the DPS. The total heat tot capacity, CV , of FeSb3, obtained by combining the partial CV for Fe and Sb obtained from tot Sb Fe NIS by CV = 3 · CV + CV , are shown in Fig. 11. These values are compared with the total 16 CV of CoSb3, obtained by combining the partial CV for Co from calculations and for Sb from NIS measurements, measurements that are in good agreement with the calculation in

Ref. 16. Also a macroscopic CP measurement of CoSb3, carried out with the CP option of the QD-PPMS that is in excellent agreement with earlier results39, is also shown. With a Debye

ﬁt of the CV between 2 and 300 K, Debye temperatures for Sb and Fe in FeSb3 of 210(5) and 430(10) K, respectively, have been obtained, values that are in good agreement with tot those obtained by diﬀraction, see TableIII. From CV for FeSb3, a Debye temperature of

240(10) K has been obtained. The partial CV of CoSb3 yields Debye temperatures of 250(5) and 410(10) K for Sb and Co, respectively. The total Debye temperature of CoSb3 from the macroscopic measurement is 280(10) K, in good agreement with the θD = 285(10) K 121 obtained from the combined experimental Sb NIS CV and the theoretical Co CV . Chapter 2: FeSb3 – Nuclear resonance scattering 42

200 8000 6000 I 100 4000

2000 NFS (a.u.) 0 0 FeSb3 600 Fe 1200 Sb 400 800 200 400 0 0 600 CoSb3 Sb 1200 NIS (counts) NFS (counts) 400 800

200 400 (a.u.)

I 0 0 EuFe4Sb12 600 Sb 300 I (NFS) 400 200 200 100 (a.u.) 0 0 I -10 0 10 20 30 40

E (meV) I (NFS)

FIG. 9. The nuclear inelastic scattering, NIS, spectra and the instrumental functions, dashed lines,

57 measured by nuclear forward scattering, NFS, obtained with the Fe resonance of FeSb3, top, and

121 with the Sb resonance of FeSb3, CoSb3 and EuFe4Sb12, bottom.

2 From the Debye level, limE→0(g(E)/E ), obtained from the low energy modes in the reduced DPS, see the insets to Fig. 10, the average velocity of sound, vs, of 2390(10) and 57 2790(10) m/s for FeSb3 and EuFe4Sb12, respectively, was obtained from the Fe NIS by using47

2 mR lim(g(E)/E ) = 2 3 3 (1) E→0 2π ρ~ vs

where ρ is the density of the material and mR the mass of the resonant nucleus. These veloc-

ities of sound are consistent with the Sb Debye level in FeSb3 and EuFe4Sb12, as indicated by

the dashed lines in the insets to Fig. 10, see also TableIII. For CoSb 3 a vs of 2600(100) m/s is obtained from the Debye level, in fair agreement with the literature value28 of 2930 m/s. Chapter 2: FeSb3 – Nuclear resonance scattering 43

FeSb3 0.15 EuFe4Sb12

2

0.10

(1/meV) 1 g(E)

0 Fe, 0.05

57 0 10 20

0.00 FeSb3 0.15 CoSb3 EuFe4Sb12 8

6 0.10 (1/meV) 4 g(E) Sb, 0.05 2 121 0 10

0.00 0 5 10 15 20 25 30 35 40 E (meV)

57 FIG. 10. Comparison of the DPS measured with the Fe resonance at 300 K for FeSb3 and

121 EuFe4Sb12, top, and with the Sb resonance at 25 K for FeSb3, CoSb3, and EuFe4Sb12, bottom. The insets show the reduced partial DPS, g(E)/(E2), in units of 10−4/meV3 and the low energy ﬁt, between 0 and 4 meV, for the Debye levels, indicated by the same type of lines. The diﬀerences in the Debye levels for Fe and Sb in FeSb3 and EuFe4Sb12 are due to the diﬀerent masses of the elements, see Eq.1. Chapter 2: FeSb3 – Nuclear resonance scattering 44

100 FeSb3, DPS CoSb3, DPS CoSb , macro. 80 3

60 5 100 10 x

(J/(K mol)) 40 10 V mol)) 4 C

20 (J/(K 1 3 /T V

C 10 100 0 0 100 200 300 T (K)

FIG. 11. A comparison of the total heat capacity, calculated from the DPS of FeSb3, red, the total heat capacity, calculated from the DPS and theoretical calculations for CoSb3, green, and the macroscopic measured heat capacity of CoSb3, blue.

The large error arises from the imprecision in the Debye level obtained only from the 121Sb 2 1/3 NIS. By using the low temperature Debye approximation, vs = (kBθD)/(~(6π N) ), with LT the density of atoms N, the low temperature θD = 245(5) K is obtained for FeSb3, a value LT signiﬁcantly lower than θD = 307 K reported for CoSb3 [39].

The Lamb-M¨ossbauerfactor, fLM , obtained from NIS provides access to the atomic mean 2 2 20 square displacements, hu i = −ln(fLM )/k , where k is the incident wavevector . In FeSb3 Sb 2 ˚2 Fe 2 the fLM is 0.58(1) and hu i is 0.0015(5) A for Sb at 25 K and fLM is 0.733(5) and hu i is 0.0057(4) A˚2 for Fe at 295 K. These values are much smaller than the hu2i values obtained by diﬀraction, see Fig.7. Note that the displacement parameter obtained by NIS is a purely incoherent one particle displacement and is not aﬀected by the site occupation or disorder as the hu2i values obtained from diﬀraction sometimes are aﬀected. The temperature de- pendence of hu2i obtained from the DPS20, see Fig.7, is in agreement with the temperature dependence of hu2i obtained by diﬀraction, apart from an additive constant, which reﬂects a static displacement, or a site disorder, or an incomplete site occupation. The element speciﬁc Debye temperatures can also be calculated directly from g(E) with the expression Chapter 2: FeSb3 – Nuclear resonance scattering 45

∞ 2 2 R 2 θD = 3/(kB g(E)dE/E ) obtained in the high temperature limit, see Ref. [20]. For FeSb3 0 Debye temperatures of 210(10) K for Sb and 370(5) K for Fe were obtained; the average value of 255(5) K is in agreement with 245(5) and 240(10) K obtained from sound velocity and CV , respectively. The element speciﬁc Debye temperature in CoSb3 was obtained from the measured 121Sb DPS, 245(5) K, and from the theoretical Co DPS16, 360(10) K. In or- der to provide an easy comparison between the results of the diﬀerent methods, we give a summary of all the Debye temperatures in TableIII. Arguably, the Debye temperature is a crude approximation, but allows straightforward comparison. In essence, we observe that the Sb sublattice is systematically softer in FeSb3, whereas the Fe sublattice in FeSb3 is harder than the Co sublattice in CoSb3.

The DPS obtained from NIS also directly yields20 the element speciﬁc mean force con- ∞ m R 2 stants, F = mR/~ g(E)E dE. The mean force constant of 160(10) N/m for Sb in CoSb3 0 is larger than the values of 105(5) and 100(10) N/m observed for FeSb3 and EuFe4Sb12, re- spectively, because the high energy optical phonon modes of the ﬁlled structure are similar to FeSb3, whereas in CoSb3 they have a larger energy. The Sb force constant in CoSb3 de- viates from the literature value of 117 N/m, obtained from earlier NIS measurements17 and 119 N/m, the mean force constant of Sb obtained from calculations16. This deviation can be ascribed essentially to the better resolution and more precise energy calibration available herein22. Thus, the good agreement obtained earlier16,17 is not conﬁrmed herein and the experimental mean force constant in CoSb3 appears to be larger than the calculated value. m The Sb mean force constant for EuFe4Sb12 is in good agreement with the F obtained from 17 previous NIS measurements . This indicates, that by ﬁlling FeSb3 with Eu, the average Sb binding does not change. Further, CoSb3 has very diﬀerent Sb lattice dynamics and thus is not an ideal compound for investigating the inﬂuence of ﬁlling upon the lattice dynamics of the RFe4Sb12 compounds. In FeSb3 the Fe mean force constant is 186(1) N/m, a value 16 close to the value of 190(4) N/m in EuFe4Sb12. The calculated mean force constant for

Co in CoSb3 of 176 N/m is slightly smaller, indicating a softer Co binding in the [Co4Sb12] framework as compared to the Fe binding in the [Fe4Sb12] framework. Chapter 2: FeSb3 – Conclusion 46

TABLE III. Summary of the Debye temperatures and the sound velocities in FeSb3 and CoSb3 obtained by diﬀerent techniques.

av a) obtained from θD = (3 · θD,Sb + θD,Fe/Co)/4, b) obtained from reference [16], c) from reference [39], d) from reference [28]

Technique FeSb3 CoSb3

av av θD,Sb,K θD,Fe,K θD ,K θD,Sb,K θD,Co,K θD ,K hu2i, XRD 230(5) 410(10) 275(5)a 280(10) 380(30) 305(15)a M¨ossbauerspectral area 1.5 µm - 350(5) - --- Heat capacity DPS 210(5) 430(10) 240(10) 250(5) 410(10)b 285(10) Heat capacity macroscopic --- - - 280(10) DPS 210(10) 370(5) 255(5)a 245(5) 360(10)b 270(10)a

c θD form vs - - 245(5) - - 307

av av vs,Sb, m/s vs,Fe, m/s vs , m/s vs,Sb, m/s vs,Co, m/s vs , m/s NIS, Debye level 2400(100) 2390(10) - 2600(100) - - Pulse echo --- - - 2930d

IV. CONCLUSION

The magnetic and electric properties of FeSb3 reveal semiconducting and paramagnetic

behavior similar to CoSb3, with however a larger eﬀective paramagnetic moment. X-ray diﬀraction and M¨ossbauerspectral measurements reveal that the sample is single phase. Measurements of the lattice dynamics and the related quantities show that the Sb binding

in FeSb3 is signiﬁcantly softer than in CoSb3, whereas the Fe sublattice in FeSb3 is harder

compared to the Co sublattice in CoSb3. The softening of the low energy modes likely has a large inﬂuence on the thermal conductivity and thus favorably impacts the thermoelectric

properties in FeSb3. By ﬁlling the [Fe4Sb12] framework, the low energy optical phonon modes, which have mainly Sb character, shift to larger energies. The lattice dynamics in ﬁlled

skutterudites depends both on the framework and the ﬁller and therefore the [Co4Sb12]

framework is not ideal to study the inﬂuence of the ﬁller on the lattice dynamics in RFe4Sb12 skutterudites. It appears that for skutterudites, as was also suggested for clathrates48, the role of the framework on the lattice dynamics should be revisited. Chapter 2: FeSb3 47

ACKNOWLEDGMENTS

We thank Dr. H.-C. Wille and Mr. D. Bessas for their support during the NIS measure- ments and Dr. J.C. Feldman for making his calculation data16 available. We thank Dr. B.C. 17 Sales for providing the CoSb3 and EuFe4Sb12 samples . The European Synchrotron Radia- tion Facility and the Advanced Photon Source are acknowledged for provision of synchrotron radiation beam time at the nuclear resonance station ID18 and ID22N and the high en- ergy station 6-ID-D, respectively. RH acknowledges support from the Helmholtz-University Young Investigator Group ’Lattices Dynamics in Emerging Functional Materials’. FG ac- knowledges the ﬁnancial support of the Fonds National de la Recherche Scientiﬁque, Belgium (grants 9.456595 and 1.5.064.05). The research at the University of Oregon was funded by National Science Foundation under grant DMR 0907049 and supported in part by ONR Grant No. N00014-07-1-0358 and by the Army Research Laboratory under agreement num- ber W911NF-07-2-0083.

∗ [email protected] 1 J. P. Fleurial et al., Thirteenth international conference on thermoelectrics, AIP Conference proceedings 316, 40-44 (1995). 2 B. C. Sales et al., Phys. Rev. B 56, 15081-15089 (1997). 3 G. S. Nolas, D. T. Morelli, and T. M. Tritt, Annu. Rev. Mater. Sci. 29, 89-116 (1999). 4 C. Uher, Semiconductors and Semimetals 69, 139-253 (2001). 5 G. S. Nolas et al., J. Appl. Phys. 79, 4002-4008 (1995). 6 G. S. Nolas, J. L. Cohn, and G. A. Slack, Phys. Rev. B 58, 164-170 (1998). 7 G. P. Meisner et al., Phys. Rev. Lett. 80, 3551-3554 (1998). 8 J. L. Feldman, and D. J. Singh, Phys. Rev. B 53, 6273-6282 (1996). 9 V. Keppens et al., Nature 395, 876-878 (1998). 10 R. P. Hermann et al., Phys. Rev. Lett. 90, 135505 (2003). 11 M. M. Koza et al., Nature Materials 7, 805-810 (2008). 12 M. Rotter et al., Phys. Rev. B 77, 144301 (2008). 13 B. C. Sales, B. C. Chakoumakos, and D. Mandrus, Phys. Rev. B 61, 2475-2481 (2000). Chapter 2: FeSb3 48

14 C. Uher, Thermoelectrics Handbook: Macro to nano (Taylor & Francis Group, LLC, 2006). 15 J. Yang et al., Phys. Rev. B 80, 115329 (2009). 16 J. L. Feldman et al., Phys. Rev. B 73, 014306 (2006). 17 H. C. Wille et al., Phys. Rev. B 76, 140301(R) (2007). 18 M. D. Hornbostel et al., J. Am. Chem. Soc. 119, 2665-2668 (1997). 19 J. R. Williams, M. B. Johnson, and D. C. Johnson, J. Am. Chem. Soc. 123, 1645-1649 (2001). 20 R. R¨uﬀer,and A. I. Chumakov, Hyp. Interact. 128, 225-272 (2000). 21 W. Sturhahn et al., Phys. Rev. Lett. 74, 3832-3835 (1995). 22 I. Sergueev et al., J. Synch. Rad., under review (2011). 23 M. Noh, J. Thiel, and D. C. Johnson, Science 270, 1181-1184 (1995). 24 A. P. Hammersley, ESRF Internal Report, ESRF97HA02T, ’FIT2D: An Introduction and Overview’, (1997). 25 J. Rodriguez-Carvajal, FULLPROF V (2009)(Laboratoire Leon Brillouin (CEA-CNRS), France, 2009). 26 D. Mandrus et al., Phys. Rev. B 52, 4926-4931 (1995). 27 H. Anno et al., J. Appl. Phys. 83, 5270-5276 (1998). 28 T. Caillat, A. Borshchevsky, and J. P. Fleurial, J. Appl. Phys. 80, 4442-4449 (1996). 29 L. D. Chen et al., J. Appl. Phys. 90, 1864 (2001). 30 M. Puyet et al., Phys. Rev. B 73, 035126 (2006). 31 A. L. E. Smalley, S. Kim, and D. C. Johnson, Chem. Mater. 15, 3847-3851 (2003). 32 J. Yang et al., Phys. Rev. B 63, 014410 (2000). 33 J. Yang, M. G. Endres, and G. P. Meisner, Phys. Rev. B 66, 014436 (2002). 34 T. Rosenqvist, Acta Metallurgica 1, 761-763 (1953). 35 G. Rogl et al., J. Appl. Phys. 107, 043507 (2010). 36 L. Zhang et al., Mat. Sci. Eng. B 170, 26-31 (2010). 37 D. T. Morelli, V. Jovovic, and J. P. Heremans, Phys. Rev. Lett. 101, 035901 (2008). 38 B. T. M. Willis and A.W. Pryor, Thermal Vibrations in Crystallography (Cambridge University Press, 1975). 39 R. P. Hermann, F. Grandjean, and G. J. Long, Am. J. Phys. 73, 110-118 (2005). 40 B. C. Chakoumakos, and B. C. Sales, J. Alloys Compd. 407, 87-93 (2006). Chapter 2: FeSb3 49

41 R. H. Herber in Chemical M¨ossbauer Spectroscopy, edited by R. H. Herber, p.199 (Plenum Press New York, 1984). 42 G. K. Shenoy and F. E. Wagner, M¨ossbauer Isomer Shifts, p.49 (North-Holland, Amsterdam, 1978). 43 T. Owen et al., Inorg. Chem. 47, 8704-8713 (2008). 44 V. G. Kohn, and A. I. Chumakov, Hyp. Interact. 125, 205-221 (2000). 45 H. J. Lipkin, Phys. Rev. B 52, 10073 (1995). 46 G. J. Long et al., Phys. Rev. B 71, 140302 (2005). 47 M. Y. Hu et al., Phys. Rev. B 67, 094304 (2003). 48 M. Christensen et al., J. Am. Chem. Soc. 128, 15657-15665 (2006). 118 Conclusions and Outlook

The lattice dynamics in thermoelectric Zintl phases were studied by inelastic neutron scatter- ing, nuclear inelastic scattering and several macroscopic techniques. Combining the results obtained by these methods, a detailed insight into the lattice dynamics and the diﬀerent mechanisms which lead to the low thermal conductivity in thermoelectric Zintl phases was obtained. The knowledge of these thermal conductivity reduction mechanisms will prove useful in order to search for and enhance new eﬃcient thermoelectric materials. The main mechanisms in the studied Zintl phases are the reduction of the phonon lifetime by the ﬁller, the reduction of the phonon velocity by the ﬁller or a low velocity of sound, and the reduction of the eﬀective heat capacity contribution due to a complex crystal structure.

It was shown, that the skutterudite FeSb3 is signiﬁcantly softer than the isostructural

compound CoSb3. Thus, beside the reduction of the thermal conductivity by the ﬁller,

the low thermal conductivity in the ﬁlled skutterudite RFe4Sb12 is also related to the soft

[Fe4Sb12] framework. Furthermore, it was shown, that the lattice dynamics of the [Fe4Sb12] framework is only slightly aﬀected by ﬁlling the structure. Several mechanisms are responsible for the low thermal conductivity in Ga-Ge clathrates. The reduction of the heat capacity contribution to the thermal conductivity due to the large unit cell of the clathrate structure is one additional mechanism next to the small phonon lifetime and the low phonon group velocity, which are both related to the guest atoms. Fur- thermore, the predicted avoided crossing in Ga-Ge clathrates was modeled and the inﬂuence on the thermal conductivity was investigated. This study reveals, that an avoided crossing could lower the thermal conductivity by up to 30%.

The scattering experiments reveal that in the Zintl phase Yb14MnSb11 all phonon modes have energies below 25 meV, which is in agreement with the low Debye temperature. The low mean force constants, and the related low velocity of sound, are one reason for the low thermal conductivity in Yb14MnSb11. Furthermore, Yb14MnSb11 has a rather large unit cell. Therefore the acoustic modes involve a small fraction of the heat capacity and contribute less eﬃciently to the thermal conductivity.

119 Several questions are opened for further investigations:

First, it was shown that the lattice dynamics in RFe4Sb12 skutterudites depend both on the

[Fe4Sb12] framework and on the ﬁller and the lattice dynamics in the [Fe4Sb12] framework changes only slightly when ﬁlling the structure. Thus, the inﬂuence of the ﬁller and the framework to the lattice dynamics and the thermal conductivity should be revisited.

Second, further studies on the change of the Yb valence state in YbFe4Sb12 with the tem- perature should be carried out and the inﬂuence of the related anomalous softening in the elastic constants and the rearrangement of the spectral weight of the Yb phonon states to the thermoelectric properties should be investigated and modeled quantitatively. Third, this study reveals, that in complex crystal structures the reduction of the heat capac- ity contribution to the thermal conductivity is an important mechanism for the low thermal conductivity. In order to clarify this reduction both theoretical calculations and further ex- perimental studies of the phonon dispersion have to be carried out. Fourth, in order to reveal, if an avoided crossing takes place in Ga-Ge clathrates, more theoretical calculations are required. In particular a quantitative modeling of the inelastic neutron scattering with the dynamical structure factor will bring deeper insight into the lattice dynamics and the mechanisms which lead to the low thermal conductivity in Ga-Ge clathrates.

120 121 Vita

Anne M¨ochel was born on the 27th August 1982 in Bremerhaven, Germany. She received her Abitur, German university entrance qualiﬁcation, at the Schulzentrum B¨urgermeister Smidt in Bremerhaven, Germany, in 2002. She received her diploma in Physics from the University of Bonn in 2008. She carried out her doctoral research at the Forschungszentrum J¨ulich and the University of Li`egeunder the supervision of Dr. Rapha¨elHermann.

Publications and submitted or prepared manuscripts:

1. M. Beekman, R. P. Hermann, A. M¨ochel, F. Juranyi, and G. S. Nolas, A study of

low-energy guest phonon modes in clathrate-II NaxSi136 (x = 3, 23, and 24), J. Phys.: Condens. Matter 22, 355401 (2010).

2. H.-C. Wille, R. P. Hermann, I. Sergueev, U. Pelzer, A. M¨ochel, T. Claudio, J. Perßon, R. R¨uﬀer,A. Said, and Yu. V. Shvyd’ko, Nuclear forward and inelastic spec- 125 125 troscopy on Te and Sb2 Te3, Europhys. Lett. 91, 62001 (2010).

3. A. M¨ochel, I. Sergueev, N. Nguyen, Gary J. Long, F. Grandjean, D. C. Johnson, and

R. P. Hermann, Lattice Dynamics in the FeSb3 Skutterudite, submitted to Phys. Rev. B, March 2011.

4. J. Burghaus, M. Sougrati, A. M¨ochel, A. Houben, R. P. Hermann, and R. Dronskowski,

Local ordering and magnetism in Ga0.9Fe3.1N, submitted to Phys. Chem. Chem. Phys., April 2011.

5. M. S. Diakhate, R. P. Hermann, A. M¨ochel, I. Sergueev, M. Søndergaard, M. Chris- tensen and M. J. Verstraete, Thermodynamic, thermoelectric and magnetic

properties of FeSb2: A combined ﬁrst principles and experimental study, submitted to Phys. Rev. B, May 2011.

6. A. M¨ochel, I. Sergueev, H.-C. Wille, F. Juranyi, H. Schober, W. Schweika, S. R. Brown, S. M. Kauzlarich, and R. P. Hermann, Lattice dynamics in the thermoelectric

Zintl compound Yb14MnSb11, to be submitted to Phys. Rev. B, May 2011.

122 7. A. M¨ochel, I. Sergueev, H.-C. Wille, J. Voigt, M. Prager, M. B. Stone, B. C. Sales, Z. Guguchia, A. Shengelaya, V. Keppens, and R. P. Hermann, Lattice dynamics

and anomalous softening in the YbFe4Sb12 skutterudite, to be submitted to Phys. Rev. B, May 2011.

8. A. M¨ochel, W. Schweika, K. Schmalzl, B. C. Sales, and R. P. Hermann, Experimental

study of the phonon dispersion in the Sr8Ga16Ge30 clathrate, to be submitted to New Journ. Phys., June 2011.

123